# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_crystal
_database_code_depnum_ccdc_archive 'CCDC 2207869'
loop_
_audit_author_name
_audit_author_address
'Linfang Xie'
;Shandong University
China
;
_audit_update_record             
;
2022-09-17 deposited with the CCDC.	2022-10-31 downloaded from the CCDC.
;


_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Ca2 Nb2 O7'
_chemical_formula_sum            'Ca2 Nb2 O7'
_chemical_formula_weight         377.98

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'Pna2(1) '

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'x+1/2, -y+1/2, z'

_cell_length_a                   26.470(3)
_cell_length_b                   7.6950(7)
_cell_length_c                   5.4985(5)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     1119.95(18)
_cell_formula_units_Z            8
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    2084
_cell_measurement_theta_min      3.08
_cell_measurement_theta_max      27.51

_exptl_crystal_description       plate
_exptl_crystal_colour            colourless
_exptl_crystal_size_max          0.13
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.05
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.483
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1424
_exptl_absorpt_coefficient_mu    5.906
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.5140
_exptl_absorpt_correction_T_max  0.7567
_exptl_absorpt_process_details   'APEX2 Software Suite (Bruker,2009)'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker APEX2 CCD area-detector diffractometer'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count .
_diffrn_standards_interval_time  .
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            6580
_diffrn_reflns_av_R_equivalents  0.0201
_diffrn_reflns_av_sigmaI/netI    0.0244
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_h_max       31
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_theta_min         2.76
_diffrn_reflns_theta_max         27.51
_reflns_number_total             2515
_reflns_number_gt                2074
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'APEX2 Software Suite (Bruker,2009)'
_computing_cell_refinement       'APEX2 Software Suite (Bruker,2009)'
_computing_data_reduction        'APEX2 Software Suite (Bruker,2009)'
_computing_structure_solution    'SIR97 (Altomare,1999)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'SHELXTL (Bruker, 1997)'
_computing_publication_material  'WINGX (Farrugia,1999)'

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0225P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00041(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.02(5)
_refine_ls_number_reflns         2515
_refine_ls_number_parameters     200
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0268
_refine_ls_R_factor_gt           0.0208
_refine_ls_wR_factor_ref         0.0525
_refine_ls_wR_factor_gt          0.0489
_refine_ls_goodness_of_fit_ref   1.023
_refine_ls_restrained_S_all      1.023
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Nb3 Nb 0.087128(11) 0.36890(4) 0.62169(7) 0.00532(9) Uani 1 1 d . . .
Nb2 Nb 0.191338(11) 0.37742(4) 0.14765(7) 0.00437(9) Uani 1 1 d . . .
Nb4 Nb 0.088537(11) 0.87706(4) -0.37422(7) 0.00499(9) Uani 1 1 d . . .
Nb1 Nb 0.192482(11) -0.12942(4) 0.14618(7) 0.00455(9) Uani 1 1 d . . .
Ca1 Ca 0.20516(3) 0.12327(9) -0.3528(2) 0.00924(17) Uani 1 1 d . . .
Ca4 Ca 0.03423(3) 1.12345(10) -0.9359(2) 0.00912(18) Uani 1 1 d . . .
Ca2 Ca 0.18991(3) 0.62311(9) 0.65731(19) 0.00820(17) Uani 1 1 d . . .
Ca3 Ca 0.05133(3) 0.61810(10) 0.1311(2) 0.01369(18) Uani 1 1 d . . .
O11 O 0.03661(11) 0.8477(4) -0.1545(6) 0.0109(7) Uani 1 1 d . . .
O4 O 0.23966(10) 0.4151(3) -0.1242(6) 0.0085(6) Uani 1 1 d . . .
O7 O 0.16050(10) 0.3492(3) 0.4655(5) 0.0075(6) Uani 1 1 d . . .
O6 O 0.26030(10) 0.3330(3) 0.3741(6) 0.0099(6) Uani 1 1 d . . .
O8 O 0.05673(10) 0.3397(4) 0.3350(5) 0.0104(7) Uani 1 1 d . . .
O3 O 0.19556(9) 0.1239(3) 0.0832(6) 0.0103(7) Uani 1 1 d . . .
O14 O 0.04834(11) 0.9025(4) -0.6431(6) 0.0095(6) Uani 1 1 d . . .
O9 O 0.09831(10) 0.1240(3) 0.7270(6) 0.0098(6) Uani 1 1 d . . .
O10 O 0.03129(10) 0.3947(4) 0.8261(6) 0.0098(7) Uani 1 1 d . . .
O2 O 0.13780(10) -0.1837(4) -0.0463(5) 0.0109(6) Uani 1 1 d . . .
O5 O 0.13666(10) 0.4318(4) -0.0450(5) 0.0101(6) Uani 1 1 d . . .
O13 O 0.15967(10) 0.8995(3) -0.5360(5) 0.0079(6) Uani 1 1 d . . .
O12 O 0.09895(9) 0.6236(3) -0.4389(6) 0.0094(6) Uani 1 1 d . . .
O1 O 0.20678(9) -0.3757(3) 0.2425(6) 0.0081(6) Uani 1 1 d . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Nb3 O8 1.784(3) . ?
Nb3 O10 1.868(3) . ?
Nb3 O9 1.994(3) . ?
Nb3 O12 2.013(2) 1_556 ?
Nb3 O7 2.129(3) . ?
Nb3 O5 2.305(3) 1_556 ?
Nb3 Ca2 3.3565(8) . ?
Nb3 Ca4 3.3831(11) 1_547 ?
Nb3 Ca3 3.4427(13) . ?
Nb3 Ca3 3.5243(13) 1_556 ?
Nb3 Ca1 3.6543(8) 1_556 ?
Nb3 Ca3 3.6665(9) 2_565 ?
Nb2 O5 1.842(3) . ?
Nb2 O7 1.941(3) . ?
Nb2 O3 1.986(2) . ?
Nb2 O4 1.989(3) . ?
Nb2 O1 2.012(3) 1_565 ?
Nb2 O6 2.236(3) . ?
Nb2 Ca2 3.2932(11) 1_554 ?
Nb2 Ca1 3.3293(8) 3 ?
Nb2 Ca2 3.3807(11) . ?
Nb2 Ca1 3.3918(11) 1_556 ?
Nb2 Ca1 3.3956(11) . ?
Nb2 Ca2 3.7031(9) 3_544 ?
Nb4 O14 1.832(3) . ?
Nb4 O11 1.844(3) . ?
Nb4 O9 1.997(3) 1_564 ?
Nb4 O12 2.001(2) . ?
Nb4 O13 2.090(3) . ?
Nb4 O2 2.274(3) 1_565 ?
Nb4 Ca4 3.2672(9) 2_575 ?
Nb4 Ca2 3.3240(8) 1_554 ?
Nb4 Ca4 3.3867(11) 1_556 ?
Nb4 Ca3 3.5128(13) 1_554 ?
Nb4 Ca3 3.5582(12) . ?
Nb4 Ca1 3.6240(8) 1_565 ?
Nb1 O2 1.841(3) . ?
Nb1 O13 1.964(3) 1_546 ?
Nb1 O6 1.971(3) 3_544 ?
Nb1 O3 1.982(2) . ?
Nb1 O1 2.004(3) . ?
Nb1 O4 2.222(3) 3_545 ?
Nb1 Ca2 3.2949(11) 1_544 ?
Nb1 Ca1 3.3108(8) 3_545 ?
Nb1 Ca1 3.3794(11) . ?
Nb1 Ca1 3.3888(11) 1_556 ?
Nb1 Ca2 3.3955(11) 1_545 ?
Nb1 Ca2 3.6703(9) 3_544 ?
Ca1 O7 2.328(3) 1_554 ?
Ca1 O13 2.330(3) 1_545 ?
Ca1 O1 2.389(3) 3_554 ?
Ca1 O3 2.411(3) . ?
Ca1 O4 2.632(3) 3_544 ?
Ca1 O6 2.644(3) 1_554 ?
Ca1 O6 2.717(3) 3_544 ?
Ca1 O4 2.731(3) . ?
Ca1 O9 2.862(3) 1_554 ?
Ca1 O3 3.112(3) 1_554 ?
Ca1 Nb1 3.3108(8) 3_554 ?
Ca1 Nb2 3.3293(8) 3_544 ?
Ca4 O8 2.311(3) 1_564 ?
Ca4 O14 2.371(3) . ?
Ca4 O11 2.439(3) 1_554 ?
Ca4 O11 2.441(3) 2_574 ?
Ca4 O10 2.465(3) 1_563 ?
Ca4 O14 2.473(3) 2_574 ?
Ca4 O9 2.513(3) 1_563 ?
Ca4 Nb4 3.2672(9) 2_574 ?
Ca4 Nb3 3.3832(11) 1_563 ?
Ca4 Nb4 3.3867(11) 1_554 ?
Ca4 Ca4 3.8015(11) 2_574 ?
Ca4 Ca4 3.8015(11) 2_575 ?
Ca2 O1 2.324(3) 1_565 ?
Ca2 O4 2.396(3) 1_556 ?
Ca2 O6 2.401(3) 3 ?
Ca2 O12 2.465(3) 1_556 ?
Ca2 O7 2.482(3) . ?
Ca2 O13 2.509(3) 1_556 ?
Ca2 O2 2.602(3) 1_566 ?
Ca2 O5 2.614(3) 1_556 ?
Ca2 O3 3.059(3) 3 ?
Ca2 Nb2 3.2932(11) 1_556 ?
Ca2 Nb1 3.2949(11) 1_566 ?
Ca2 Nb4 3.3240(8) 1_556 ?
Ca3 O11 2.396(3) . ?
Ca3 O8 2.422(3) . ?
Ca3 O10 2.438(3) 2_564 ?
Ca3 O10 2.459(3) 1_554 ?
Ca3 O14 2.517(3) 1_556 ?
Ca3 O12 2.680(3) 1_556 ?
Ca3 O5 2.845(3) . ?
Ca3 O2 2.918(3) 1_565 ?
Ca3 Nb4 3.5128(13) 1_556 ?
Ca3 Nb3 3.5243(13) 1_554 ?
O11 Ca4 2.439(3) 1_556 ?
O11 Ca4 2.441(3) 2_575 ?
O4 Nb1 2.222(3) 3_554 ?
O4 Ca2 2.396(3) 1_554 ?
O4 Ca1 2.632(3) 3 ?
O7 Ca1 2.328(3) 1_556 ?
O6 Nb1 1.971(3) 3 ?
O6 Ca2 2.401(3) 3_544 ?
O6 Ca1 2.644(3) 1_556 ?
O6 Ca1 2.717(3) 3 ?
O8 Ca4 2.311(3) 1_546 ?
O3 Ca2 3.059(3) 3_544 ?
O3 Ca1 3.112(3) 1_556 ?
O14 Ca4 2.473(3) 2_575 ?
O14 Ca3 2.517(3) 1_554 ?
O9 Nb4 1.997(3) 1_546 ?
O9 Ca4 2.513(3) 1_547 ?
O9 Ca1 2.862(3) 1_556 ?
O10 Ca3 2.438(3) 2_565 ?
O10 Ca3 2.459(3) 1_556 ?
O10 Ca4 2.465(3) 1_547 ?
O2 Nb4 2.274(3) 1_545 ?
O2 Ca2 2.602(3) 1_544 ?
O2 Ca3 2.918(3) 1_545 ?
O5 Nb3 2.305(3) 1_554 ?
O5 Ca2 2.614(3) 1_554 ?
O13 Nb1 1.964(3) 1_564 ?
O13 Ca1 2.330(3) 1_565 ?
O13 Ca2 2.509(3) 1_554 ?
O12 Nb3 2.013(2) 1_554 ?
O12 Ca2 2.465(3) 1_554 ?
O12 Ca3 2.680(3) 1_554 ?
O1 Nb2 2.012(3) 1_545 ?
O1 Ca2 2.324(3) 1_545 ?
O1 Ca1 2.389(3) 3_545 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O8 Nb3 O10 100.86(13) . . ?
O8 Nb3 O9 101.79(12) . . ?
O10 Nb3 O9 92.48(12) . . ?
O8 Nb3 O12 92.67(13) . 1_556 ?
O10 Nb3 O12 96.85(12) . 1_556 ?
O9 Nb3 O12 161.02(12) . 1_556 ?
O8 Nb3 O7 92.63(12) . . ?
O10 Nb3 O7 166.50(12) . . ?
O9 Nb3 O7 85.08(11) . . ?
O12 Nb3 O7 82.00(10) 1_556 . ?
O8 Nb3 O5 170.27(12) . 1_556 ?
O10 Nb3 O5 87.09(12) . 1_556 ?
O9 Nb3 O5 83.29(11) . 1_556 ?
O12 Nb3 O5 80.72(11) 1_556 1_556 ?
O7 Nb3 O5 79.45(10) . 1_556 ?
O8 Nb3 Ca2 119.38(9) . . ?
O10 Nb3 Ca2 122.98(9) . . ?
O9 Nb3 Ca2 114.43(8) . . ?
O12 Nb3 Ca2 46.85(7) 1_556 . ?
O7 Nb3 Ca2 47.60(7) . . ?
O5 Nb3 Ca2 50.96(7) 1_556 . ?
O8 Nb3 Ca4 112.23(9) . 1_547 ?
O10 Nb3 Ca4 45.49(9) . 1_547 ?
O9 Nb3 Ca4 47.54(8) . 1_547 ?
O12 Nb3 Ca4 136.65(9) 1_556 1_547 ?
O7 Nb3 Ca4 128.89(7) . 1_547 ?
O5 Nb3 Ca4 77.34(7) 1_556 1_547 ?
Ca2 Nb3 Ca4 128.23(3) . 1_547 ?
O8 Nb3 Ca3 41.73(9) . . ?
O10 Nb3 Ca3 101.22(9) . . ?
O9 Nb3 Ca3 142.65(9) . . ?
O12 Nb3 Ca3 50.99(9) 1_556 . ?
O7 Nb3 Ca3 88.55(8) . . ?
O5 Nb3 Ca3 131.51(7) 1_556 . ?
Ca2 Nb3 Ca3 86.80(2) . . ?
Ca4 Nb3 Ca3 139.50(2) 1_547 . ?
O8 Nb3 Ca3 130.51(9) . 1_556 ?
O10 Nb3 Ca3 41.49(9) . 1_556 ?
O9 Nb3 Ca3 108.88(10) . 1_556 ?
O12 Nb3 Ca3 69.12(9) 1_556 1_556 ?
O7 Nb3 Ca3 127.21(8) . 1_556 ?
O5 Nb3 Ca3 53.61(7) 1_556 1_556 ?
Ca2 Nb3 Ca3 81.63(2) . 1_556 ?
Ca4 Nb3 Ca3 67.73(3) 1_547 1_556 ?
Ca3 Nb3 Ca3 104.22(2) . 1_556 ?
O8 Nb3 Ca1 110.75(9) . 1_556 ?
O10 Nb3 Ca1 135.11(10) . 1_556 ?
O9 Nb3 Ca1 51.17(7) . 1_556 ?
O12 Nb3 Ca1 112.16(7) 1_556 1_556 ?
O7 Nb3 Ca1 36.74(7) . 1_556 ?
O5 Nb3 Ca1 65.90(7) 1_556 1_556 ?
Ca2 Nb3 Ca1 66.809(19) . 1_556 ?
Ca4 Nb3 Ca1 92.15(2) 1_547 1_556 ?
Ca3 Nb3 Ca1 123.61(3) . 1_556 ?
Ca3 Nb3 Ca1 118.74(3) 1_556 1_556 ?
O8 Nb3 Ca3 64.23(9) . 2_565 ?
O10 Nb3 Ca3 36.64(9) . 2_565 ?
O9 Nb3 Ca3 99.79(8) . 2_565 ?
O12 Nb3 Ca3 97.54(7) 1_556 2_565 ?
O7 Nb3 Ca3 156.84(8) . 2_565 ?
O5 Nb3 Ca3 123.48(7) 1_556 2_565 ?
Ca2 Nb3 Ca3 142.506(19) . 2_565 ?
Ca4 Nb3 Ca3 65.88(2) 1_547 2_565 ?
Ca3 Nb3 Ca3 73.78(2) . 2_565 ?
Ca3 Nb3 Ca3 72.85(2) 1_556 2_565 ?
Ca1 Nb3 Ca3 150.24(2) 1_556 2_565 ?
O5 Nb2 O7 102.29(12) . . ?
O5 Nb2 O3 99.49(12) . . ?
O7 Nb2 O3 94.26(12) . . ?
O5 Nb2 O4 92.29(12) . . ?
O7 Nb2 O4 164.49(12) . . ?
O3 Nb2 O4 88.45(11) . . ?
O5 Nb2 O1 95.40(12) . 1_565 ?
O7 Nb2 O1 87.58(12) . 1_565 ?
O3 Nb2 O1 164.23(11) . 1_565 ?
O4 Nb2 O1 85.79(11) . 1_565 ?
O5 Nb2 O6 175.29(11) . . ?
O7 Nb2 O6 79.91(12) . . ?
O3 Nb2 O6 84.44(10) . . ?
O4 Nb2 O6 85.17(11) . . ?
O1 Nb2 O6 80.46(10) 1_565 . ?
O5 Nb2 Ca2 52.39(9) . 1_554 ?
O7 Nb2 Ca2 142.80(8) . 1_554 ?
O3 Nb2 Ca2 114.74(9) . 1_554 ?
O4 Nb2 Ca2 46.23(8) . 1_554 ?
O1 Nb2 Ca2 70.88(9) 1_565 1_554 ?
O6 Nb2 Ca2 123.58(8) . 1_554 ?
O5 Nb2 Ca1 121.14(9) . 3 ?
O7 Nb2 Ca1 114.22(9) . 3 ?
O3 Nb2 Ca1 120.78(7) . 3 ?
O4 Nb2 Ca1 52.22(8) . 3 ?
O1 Nb2 Ca1 45.29(7) 1_565 3 ?
O6 Nb2 Ca1 54.24(7) . 3 ?
Ca2 Nb2 Ca1 71.50(2) 1_554 3 ?
O5 Nb2 Ca2 109.93(9) . . ?
O7 Nb2 Ca2 46.50(8) . . ?
O3 Nb2 Ca2 134.25(9) . . ?
O4 Nb2 Ca2 123.28(8) . . ?
O1 Nb2 Ca2 42.21(9) 1_565 . ?
O6 Nb2 Ca2 68.47(8) . . ?
Ca2 Nb2 Ca2 110.95(2) 1_554 . ?
Ca1 Nb2 Ca2 72.06(2) 3 . ?
O5 Nb2 Ca1 132.97(9) . 1_556 ?
O7 Nb2 Ca1 41.55(8) . 1_556 ?
O3 Nb2 Ca1 64.66(9) . 1_556 ?
O4 Nb2 Ca1 128.57(8) . 1_556 ?
O1 Nb2 Ca1 108.21(9) 1_565 1_556 ?
O6 Nb2 Ca1 51.15(8) . 1_556 ?
Ca2 Nb2 Ca1 174.45(2) 1_554 1_556 ?
Ca1 Nb2 Ca1 103.85(2) 3 1_556 ?
Ca2 Nb2 Ca1 69.65(3) . 1_556 ?
O5 Nb2 Ca1 75.49(9) . . ?
O7 Nb2 Ca1 135.27(8) . . ?
O3 Nb2 Ca1 44.24(9) . . ?
O4 Nb2 Ca1 53.52(8) . . ?
O1 Nb2 Ca1 137.05(9) 1_565 . ?
O6 Nb2 Ca1 105.97(8) . . ?
Ca2 Nb2 Ca1 70.64(3) 1_554 . ?
Ca1 Nb2 Ca1 103.77(2) 3 . ?
Ca2 Nb2 Ca1 174.28(2) . . ?
Ca1 Nb2 Ca1 108.21(2) 1_556 . ?
O5 Nb2 Ca2 142.69(9) . 3_544 ?
O7 Nb2 Ca2 106.55(8) . 3_544 ?
O3 Nb2 Ca2 55.64(7) . 3_544 ?
O4 Nb2 Ca2 62.73(8) . 3_544 ?
O1 Nb2 Ca2 108.83(7) 1_565 3_544 ?
O6 Nb2 Ca2 38.57(7) . 3_544 ?
Ca2 Nb2 Ca2 108.96(2) 1_554 3_544 ?
Ca1 Nb2 Ca2 66.535(19) 3 3_544 ?
Ca2 Nb2 Ca2 107.05(2) . 3_544 ?
Ca1 Nb2 Ca2 65.926(19) 1_556 3_544 ?
Ca1 Nb2 Ca2 67.40(2) . 3_544 ?
O14 Nb4 O11 96.26(14) . . ?
O14 Nb4 O9 101.45(12) . 1_564 ?
O11 Nb4 O9 91.75(12) . 1_564 ?
O14 Nb4 O12 92.32(13) . . ?
O11 Nb4 O12 95.73(12) . . ?
O9 Nb4 O12 163.52(12) 1_564 . ?
O14 Nb4 O13 99.84(13) . . ?
O11 Nb4 O13 163.89(13) . . ?
O9 Nb4 O13 85.60(11) 1_564 . ?
O12 Nb4 O13 83.15(10) . . ?
O14 Nb4 O2 174.27(11) . 1_565 ?
O11 Nb4 O2 83.26(12) . 1_565 ?
O9 Nb4 O2 84.27(11) 1_564 1_565 ?
O12 Nb4 O2 82.06(11) . 1_565 ?
O13 Nb4 O2 80.67(10) . 1_565 ?
O14 Nb4 Ca4 48.60(10) . 2_575 ?
O11 Nb4 Ca4 47.66(10) . 2_575 ?
O9 Nb4 Ca4 99.15(8) 1_564 2_575 ?
O12 Nb4 Ca4 96.74(7) . 2_575 ?
O13 Nb4 Ca4 148.45(8) . 2_575 ?
O2 Nb4 Ca4 130.72(8) 1_565 2_575 ?
O14 Nb4 Ca2 125.01(9) . 1_554 ?
O11 Nb4 Ca2 119.71(9) . 1_554 ?
O9 Nb4 Ca2 116.12(8) 1_564 1_554 ?
O12 Nb4 Ca2 47.57(7) . 1_554 ?
O13 Nb4 Ca2 48.96(7) . 1_554 ?
O2 Nb4 Ca2 51.31(7) 1_565 1_554 ?
Ca4 Nb4 Ca2 143.86(2) 2_575 1_554 ?
O14 Nb4 Ca4 105.54(9) . 1_556 ?
O11 Nb4 Ca4 44.43(9) . 1_556 ?
O9 Nb4 Ca4 47.46(8) 1_564 1_556 ?
O12 Nb4 Ca4 136.93(9) . 1_556 ?
O13 Nb4 Ca4 129.73(8) . 1_556 ?
O2 Nb4 Ca4 78.12(8) 1_565 1_556 ?
Ca4 Nb4 Ca4 69.658(18) 2_575 1_556 ?
Ca2 Nb4 Ca4 129.39(3) 1_554 1_556 ?
O14 Nb4 Ca3 43.35(9) . 1_554 ?
O11 Nb4 Ca3 103.23(10) . 1_554 ?
O9 Nb4 Ca3 142.37(9) 1_564 1_554 ?
O12 Nb4 Ca3 49.32(9) . 1_554 ?
O13 Nb4 Ca3 88.27(8) . 1_554 ?
O2 Nb4 Ca3 131.17(7) 1_565 1_554 ?
Ca4 Nb4 Ca3 68.90(2) 2_575 1_554 ?
Ca2 Nb4 Ca3 86.17(2) 1_554 1_554 ?
Ca4 Nb4 Ca3 138.56(2) 1_556 1_554 ?
O14 Nb4 Ca3 121.95(9) . . ?
O11 Nb4 Ca3 38.13(9) . . ?
O9 Nb4 Ca3 110.56(9) 1_564 . ?
O12 Nb4 Ca3 68.36(9) . . ?
O13 Nb4 Ca3 128.91(8) . . ?
O2 Nb4 Ca3 54.86(7) 1_565 . ?
Ca4 Nb4 Ca3 78.76(2) 2_575 . ?
Ca2 Nb4 Ca3 81.57(2) 1_554 . ?
Ca4 Nb4 Ca3 68.92(3) 1_556 . ?
Ca3 Nb4 Ca3 102.08(2) 1_554 . ?
O14 Nb4 Ca1 117.72(10) . 1_565 ?
O11 Nb4 Ca1 132.66(10) . 1_565 ?
O9 Nb4 Ca1 51.91(7) 1_564 1_565 ?
O12 Nb4 Ca1 113.44(7) . 1_565 ?
O13 Nb4 Ca1 37.16(8) . 1_565 ?
O2 Nb4 Ca1 65.99(7) 1_565 1_565 ?
Ca4 Nb4 Ca1 148.35(2) 2_575 1_565 ?
Ca2 Nb4 Ca1 67.542(19) 1_554 1_565 ?
Ca4 Nb4 Ca1 92.62(2) 1_556 1_565 ?
Ca3 Nb4 Ca1 124.10(2) 1_554 1_565 ?
Ca3 Nb4 Ca1 120.21(3) . 1_565 ?
O2 Nb1 O13 100.92(12) . 1_546 ?
O2 Nb1 O6 91.67(12) . 3_544 ?
O13 Nb1 O6 166.52(12) 1_546 3_544 ?
O2 Nb1 O3 98.92(12) . . ?
O13 Nb1 O3 93.56(12) 1_546 . ?
O6 Nb1 O3 89.19(11) 3_544 . ?
O2 Nb1 O1 94.93(12) . . ?
O13 Nb1 O1 87.45(12) 1_546 . ?
O6 Nb1 O1 86.67(11) 3_544 . ?
O3 Nb1 O1 165.65(11) . . ?
O2 Nb1 O4 175.64(10) . 3_545 ?
O13 Nb1 O4 80.47(11) 1_546 3_545 ?
O6 Nb1 O4 86.63(11) 3_544 3_545 ?
O3 Nb1 O4 85.08(10) . 3_545 ?
O1 Nb1 O4 80.97(10) . 3_545 ?
O2 Nb1 Ca2 51.96(9) . 1_544 ?
O13 Nb1 Ca2 141.46(8) 1_546 1_544 ?
O6 Nb1 Ca2 46.29(8) 3_544 1_544 ?
O3 Nb1 Ca2 115.27(9) . 1_544 ?
O1 Nb1 Ca2 70.91(9) . 1_544 ?
O4 Nb1 Ca2 124.70(7) 3_545 1_544 ?
O2 Nb1 Ca1 120.94(9) . 3_545 ?
O13 Nb1 Ca1 115.17(8) 1_546 3_545 ?
O6 Nb1 Ca1 52.98(9) 3_544 3_545 ?
O3 Nb1 Ca1 122.15(7) . 3_545 ?
O1 Nb1 Ca1 45.68(7) . 3_545 ?
O4 Nb1 Ca1 54.98(7) 3_545 3_545 ?
Ca2 Nb1 Ca1 71.71(2) 1_544 3_545 ?
O2 Nb1 Ca1 75.04(9) . . ?
O13 Nb1 Ca1 134.51(8) 1_546 . ?
O6 Nb1 Ca1 53.51(8) 3_544 . ?
O3 Nb1 Ca1 44.61(9) . . ?
O1 Nb1 Ca1 137.73(9) . . ?
O4 Nb1 Ca1 106.99(8) 3_545 . ?
Ca2 Nb1 Ca1 70.87(3) 1_544 . ?
Ca1 Nb1 Ca1 104.53(2) 3_545 . ?
O2 Nb1 Ca1 132.48(9) . 1_556 ?
O13 Nb1 Ca1 41.88(8) 1_546 1_556 ?
O6 Nb1 Ca1 129.68(8) 3_544 1_556 ?
O3 Nb1 Ca1 64.75(9) . 1_556 ?
O1 Nb1 Ca1 108.00(9) . 1_556 ?
O4 Nb1 Ca1 50.92(7) 3_545 1_556 ?
Ca2 Nb1 Ca1 175.50(2) 1_544 1_556 ?
Ca1 Nb1 Ca1 104.32(2) 3_545 1_556 ?
Ca1 Nb1 Ca1 108.66(2) . 1_556 ?
O2 Nb1 Ca2 109.44(9) . 1_545 ?
O13 Nb1 Ca2 47.02(8) 1_546 1_545 ?
O6 Nb1 Ca2 123.96(8) 3_544 1_545 ?
O3 Nb1 Ca2 134.20(10) . 1_545 ?
O1 Nb1 Ca2 41.81(9) . 1_545 ?
O4 Nb1 Ca2 68.43(8) 3_545 1_545 ?
Ca2 Nb1 Ca2 110.53(2) 1_544 1_545 ?
Ca1 Nb1 Ca2 72.10(2) 3_545 1_545 ?
Ca1 Nb1 Ca2 175.29(2) . 1_545 ?
Ca1 Nb1 Ca2 69.57(3) 1_556 1_545 ?
O2 Nb1 Ca2 142.80(9) . 3_544 ?
O13 Nb1 Ca2 107.47(8) 1_546 3_544 ?
O6 Nb1 Ca2 63.42(8) 3_544 3_544 ?
O3 Nb1 Ca2 56.44(7) . 3_544 ?
O1 Nb1 Ca2 109.64(7) . 3_544 ?
O4 Nb1 Ca2 39.04(7) 3_545 3_544 ?
Ca2 Nb1 Ca2 109.70(2) 1_544 3_544 ?
Ca1 Nb1 Ca2 67.060(19) 3_545 3_544 ?
Ca1 Nb1 Ca2 67.95(2) . 3_544 ?
Ca1 Nb1 Ca2 66.336(19) 1_556 3_544 ?
Ca2 Nb1 Ca2 107.47(2) 1_545 3_544 ?
O7 Ca1 O13 95.96(10) 1_554 1_545 ?
O7 Ca1 O1 125.96(9) 1_554 3_554 ?
O13 Ca1 O1 126.97(10) 1_545 3_554 ?
O7 Ca1 O3 111.83(10) 1_554 . ?
O13 Ca1 O3 112.14(10) 1_545 . ?
O1 Ca1 O3 83.39(10) 3_554 . ?
O7 Ca1 O4 119.53(11) 1_554 3_544 ?
O13 Ca1 O4 65.91(9) 1_545 3_544 ?
O1 Ca1 O4 65.47(9) 3_554 3_544 ?
O3 Ca1 O4 128.59(9) . 3_544 ?
O7 Ca1 O6 65.21(9) 1_554 1_554 ?
O13 Ca1 O6 119.39(10) 1_545 1_554 ?
O1 Ca1 O6 65.41(9) 3_554 1_554 ?
O3 Ca1 O6 128.45(9) . 1_554 ?
O4 Ca1 O6 75.11(9) 3_544 1_554 ?
O7 Ca1 O6 169.12(9) 1_554 3_544 ?
O13 Ca1 O6 76.40(9) 1_545 3_544 ?
O1 Ca1 O6 64.77(9) 3_554 3_544 ?
O3 Ca1 O6 65.20(9) . 3_544 ?
O4 Ca1 O6 64.74(8) 3_544 3_544 ?
O6 Ca1 O6 125.23(4) 1_554 3_544 ?
O7 Ca1 O4 75.71(9) 1_554 . ?
O13 Ca1 O4 168.37(9) 1_545 . ?
O1 Ca1 O4 64.54(9) 3_554 . ?
O3 Ca1 O4 64.90(9) . . ?
O4 Ca1 O4 125.17(4) 3_544 . ?
O6 Ca1 O4 64.84(8) 1_554 . ?
O6 Ca1 O4 110.63(9) 3_544 . ?
O7 Ca1 O9 64.06(9) 1_554 1_554 ?
O13 Ca1 O9 63.70(9) 1_545 1_554 ?
O1 Ca1 O9 158.52(11) 3_554 1_554 ?
O3 Ca1 O9 75.13(9) . 1_554 ?
O4 Ca1 O9 129.53(8) 3_544 1_554 ?
O6 Ca1 O9 129.15(8) 1_554 1_554 ?
O6 Ca1 O9 105.29(8) 3_544 1_554 ?
O4 Ca1 O9 104.97(8) . 1_554 ?
O7 Ca1 O3 61.93(9) 1_554 1_554 ?
O13 Ca1 O3 61.84(8) 1_545 1_554 ?
O1 Ca1 O3 107.35(9) 3_554 1_554 ?
O3 Ca1 O3 169.26(11) . 1_554 ?
O4 Ca1 O3 58.74(8) 3_544 1_554 ?
O6 Ca1 O3 58.53(8) 1_554 1_554 ?
O6 Ca1 O3 119.10(8) 3_544 1_554 ?
O4 Ca1 O3 119.00(8) . 1_554 ?
O9 Ca1 O3 94.13(8) 1_554 1_554 ?
O7 Ca1 Nb1 89.17(7) 1_554 3_554 ?
O13 Ca1 Nb1 147.87(8) 1_545 3_554 ?
O1 Ca1 Nb1 36.88(6) 3_554 3_554 ?
O3 Ca1 Nb1 94.98(7) . 3_554 ?
O4 Ca1 Nb1 83.96(6) 3_544 3_554 ?
O6 Ca1 Nb1 36.53(6) 1_554 3_554 ?
O6 Ca1 Nb1 101.42(6) 3_544 3_554 ?
O4 Ca1 Nb1 41.80(6) . 3_554 ?
O9 Ca1 Nb1 143.88(5) 1_554 3_554 ?
O3 Ca1 Nb1 93.68(5) 1_554 3_554 ?
O7 Ca1 Nb2 147.41(8) 1_554 3_544 ?
O13 Ca1 Nb2 90.32(7) 1_545 3_544 ?
O1 Ca1 Nb2 36.76(6) 3_554 3_544 ?
O3 Ca1 Nb2 95.00(7) . 3_544 ?
O4 Ca1 Nb2 36.67(6) 3_544 3_544 ?
O6 Ca1 Nb2 83.86(6) 1_554 3_544 ?
O6 Ca1 Nb2 41.90(6) 3_544 3_544 ?
O4 Ca1 Nb2 101.06(6) . 3_544 ?
O9 Ca1 Nb2 144.50(5) 1_554 3_544 ?
O3 Ca1 Nb2 93.95(5) 1_554 3_544 ?
Nb1 Ca1 Nb2 69.713(17) 3_554 3_544 ?
O8 Ca4 O14 92.18(11) 1_564 . ?
O8 Ca4 O11 159.56(11) 1_564 1_554 ?
O14 Ca4 O11 72.94(10) . 1_554 ?
O8 Ca4 O11 73.98(10) 1_564 2_574 ?
O14 Ca4 O11 75.86(9) . 2_574 ?
O11 Ca4 O11 114.28(6) 1_554 2_574 ?
O8 Ca4 O10 74.97(10) 1_564 1_563 ?
O14 Ca4 O10 166.58(11) . 1_563 ?
O11 Ca4 O10 118.42(12) 1_554 1_563 ?
O11 Ca4 O10 103.61(9) 2_574 1_563 ?
O8 Ca4 O14 125.66(10) 1_564 2_574 ?
O14 Ca4 O14 113.22(7) . 2_574 ?
O11 Ca4 O14 74.07(9) 1_554 2_574 ?
O11 Ca4 O14 67.71(10) 2_574 2_574 ?
O10 Ca4 O14 78.22(9) 1_563 2_574 ?
O8 Ca4 O9 107.47(10) 1_564 1_563 ?
O14 Ca4 O9 113.31(10) . 1_563 ?
O11 Ca4 O9 67.69(9) 1_554 1_563 ?
O11 Ca4 O9 170.41(10) 2_574 1_563 ?
O10 Ca4 O9 68.18(9) 1_563 1_563 ?
O14 Ca4 O9 104.88(9) 2_574 1_563 ?
O8 Ca4 Nb4 100.97(7) 1_564 2_574 ?
O14 Ca4 Nb4 94.90(7) . 2_574 ?
O11 Ca4 Nb4 94.35(7) 1_554 2_574 ?
O11 Ca4 Nb4 33.94(7) 2_574 2_574 ?
O10 Ca4 Nb4 91.42(7) 1_563 2_574 ?
O14 Ca4 Nb4 33.77(7) 2_574 2_574 ?
O9 Ca4 Nb4 138.42(7) 1_563 2_574 ?
O8 Ca4 Nb3 87.41(8) 1_564 1_563 ?
O14 Ca4 Nb3 145.42(8) . 1_563 ?
O11 Ca4 Nb3 96.93(8) 1_554 1_563 ?
O11 Ca4 Nb3 136.30(8) 2_574 1_563 ?
O10 Ca4 Nb3 32.71(6) 1_563 1_563 ?
O14 Ca4 Nb3 94.56(7) 2_574 1_563 ?
O9 Ca4 Nb3 35.83(6) 1_563 1_563 ?
Nb4 Ca4 Nb3 119.14(3) 2_574 1_563 ?
O8 Ca4 Nb4 138.78(8) 1_564 1_554 ?
O14 Ca4 Nb4 90.85(8) . 1_554 ?
O11 Ca4 Nb4 31.95(7) 1_554 1_554 ?
O11 Ca4 Nb4 145.89(7) 2_574 1_554 ?
O10 Ca4 Nb4 96.30(8) 1_563 1_554 ?
O14 Ca4 Nb4 90.11(7) 2_574 1_554 ?
O9 Ca4 Nb4 35.84(6) 1_563 1_554 ?
Nb4 Ca4 Nb4 119.69(3) 2_574 1_554 ?
Nb3 Ca4 Nb4 67.98(2) 1_563 1_554 ?
O8 Ca4 Ca4 161.57(8) 1_564 2_574 ?
O14 Ca4 Ca4 101.99(8) . 2_574 ?
O11 Ca4 Ca4 38.86(7) 1_554 2_574 ?
O11 Ca4 Ca4 97.92(8) 2_574 2_574 ?
O10 Ca4 Ca4 91.39(7) 1_563 2_574 ?
O14 Ca4 Ca4 37.35(7) 2_574 2_574 ?
O9 Ca4 Ca4 77.82(6) 1_563 2_574 ?
Nb4 Ca4 Ca4 66.45(3) 2_574 2_574 ?
Nb3 Ca4 Ca4 87.494(18) 1_563 2_574 ?
Nb4 Ca4 Ca4 53.692(17) 1_554 2_574 ?
O8 Ca4 Ca4 90.95(7) 1_564 2_575 ?
O14 Ca4 Ca4 39.26(7) . 2_575 ?
O11 Ca4 Ca4 86.21(8) 1_554 2_575 ?
O11 Ca4 Ca4 38.82(7) 2_574 2_575 ?
O10 Ca4 Ca4 142.39(8) 1_563 2_575 ?
O14 Ca4 Ca4 82.62(8) 2_574 2_575 ?
O9 Ca4 Ca4 148.88(7) 1_563 2_575 ?
Nb4 Ca4 Ca4 56.65(3) 2_574 2_575 ?
Nb3 Ca4 Ca4 175.08(4) 1_563 2_575 ?
Nb4 Ca4 Ca4 115.93(3) 1_554 2_575 ?
Ca4 Ca4 Ca4 92.64(3) 2_574 2_575 ?
O1 Ca2 O4 112.90(10) 1_565 1_556 ?
O1 Ca2 O6 112.28(10) 1_565 3 ?
O4 Ca2 O6 84.18(10) 1_556 3 ?
O1 Ca2 O12 88.68(10) 1_565 1_556 ?
O4 Ca2 O12 130.21(9) 1_556 1_556 ?
O6 Ca2 O12 129.91(9) 3 1_556 ?
O1 Ca2 O7 69.30(10) 1_565 . ?
O4 Ca2 O7 79.52(9) 1_556 . ?
O6 Ca2 O7 162.58(10) 3 . ?
O12 Ca2 O7 66.67(9) 1_556 . ?
O1 Ca2 O13 69.04(9) 1_565 1_556 ?
O4 Ca2 O13 162.60(9) 1_556 1_556 ?
O6 Ca2 O13 79.36(9) 3 1_556 ?
O12 Ca2 O13 66.17(8) 1_556 1_556 ?
O7 Ca2 O13 116.09(11) . 1_556 ?
O1 Ca2 O2 135.59(10) 1_565 1_566 ?
O4 Ca2 O2 111.04(10) 1_556 1_566 ?
O6 Ca2 O2 66.15(9) 3 1_566 ?
O12 Ca2 O2 67.40(9) 1_556 1_566 ?
O7 Ca2 O2 125.82(9) . 1_566 ?
O13 Ca2 O2 67.16(9) 1_556 1_566 ?
O1 Ca2 O5 136.08(10) 1_565 1_556 ?
O4 Ca2 O5 66.80(9) 1_556 1_556 ?
O6 Ca2 O5 111.33(11) 3 1_556 ?
O12 Ca2 O5 66.97(9) 1_556 1_556 ?
O7 Ca2 O5 67.59(9) . 1_556 ?
O13 Ca2 O5 124.80(9) 1_556 1_556 ?
O2 Ca2 O5 69.13(10) 1_566 1_556 ?
O1 Ca2 O3 71.27(9) 1_565 3 ?
O4 Ca2 O3 61.53(8) 1_556 3 ?
O6 Ca2 O3 61.36(8) 3 3 ?
O12 Ca2 O3 159.95(11) 1_556 3 ?
O7 Ca2 O3 104.83(8) . 3 ?
O13 Ca2 O3 104.96(8) 1_556 3 ?
O2 Ca2 O3 127.42(9) 1_566 3 ?
O5 Ca2 O3 128.24(9) 1_556 3 ?
O1 Ca2 Nb2 143.46(7) 1_565 1_556 ?
O4 Ca2 Nb2 36.83(7) 1_556 1_556 ?
O6 Ca2 Nb2 88.47(8) 3 1_556 ?
O12 Ca2 Nb2 100.83(7) 1_556 1_556 ?
O7 Ca2 Nb2 82.18(7) . 1_556 ?
O13 Ca2 Nb2 146.85(7) 1_556 1_556 ?
O2 Ca2 Nb2 79.71(7) 1_566 1_556 ?
O5 Ca2 Nb2 33.92(6) 1_556 1_556 ?
O3 Ca2 Nb2 95.67(6) 3 1_556 ?
O1 Ca2 Nb1 142.60(7) 1_565 1_566 ?
O4 Ca2 Nb1 88.03(7) 1_556 1_566 ?
O6 Ca2 Nb1 36.39(7) 3 1_566 ?
O12 Ca2 Nb1 101.21(7) 1_556 1_566 ?
O7 Ca2 Nb1 147.56(7) . 1_566 ?
O13 Ca2 Nb1 82.08(7) 1_556 1_566 ?
O2 Ca2 Nb1 33.87(6) 1_566 1_566 ?
O5 Ca2 Nb1 79.97(7) 1_556 1_566 ?
O3 Ca2 Nb1 94.99(6) 3 1_566 ?
Nb2 Ca2 Nb1 70.34(2) 1_556 1_566 ?
O1 Ca2 Nb4 95.83(7) 1_565 1_556 ?
O4 Ca2 Nb4 149.62(8) 1_556 1_556 ?
O6 Ca2 Nb4 94.22(7) 3 1_556 ?
O12 Ca2 Nb4 36.81(6) 1_556 1_556 ?
O7 Ca2 Nb4 102.94(7) . 1_556 ?
O13 Ca2 Nb4 38.92(6) 1_556 1_556 ?
O2 Ca2 Nb4 43.01(6) 1_566 1_556 ?
O5 Ca2 Nb4 85.90(6) 1_556 1_556 ?
O3 Ca2 Nb4 142.37(5) 3 1_556 ?
Nb2 Ca2 Nb4 112.92(3) 1_556 1_556 ?
Nb1 Ca2 Nb4 73.707(19) 1_566 1_556 ?
O11 Ca3 O8 164.86(11) . . ?
O11 Ca3 O10 99.92(9) . 2_564 ?
O8 Ca3 O10 79.26(10) . 2_564 ?
O11 Ca3 O10 91.93(12) . 1_554 ?
O8 Ca3 O10 73.14(10) . 1_554 ?
O10 Ca3 O10 94.49(7) 2_564 1_554 ?
O11 Ca3 O14 71.15(11) . 1_556 ?
O8 Ca3 O14 122.86(11) . 1_556 ?
O10 Ca3 O14 77.87(9) 2_564 1_556 ?
O10 Ca3 O14 159.58(11) 1_554 1_556 ?
O11 Ca3 O12 130.02(10) . 1_556 ?
O8 Ca3 O12 65.04(9) . 1_556 ?
O10 Ca3 O12 91.98(10) 2_564 1_556 ?
O10 Ca3 O12 135.57(9) 1_554 1_556 ?
O14 Ca3 O12 64.27(9) 1_556 1_556 ?
O11 Ca3 O5 106.13(9) . . ?
O8 Ca3 O5 70.42(9) . . ?
O10 Ca3 O5 147.31(9) 2_564 . ?
O10 Ca3 O5 65.60(9) 1_554 . ?
O14 Ca3 O5 129.11(9) 1_556 . ?
O12 Ca3 O5 86.26(8) 1_556 . ?
O11 Ca3 O2 61.51(9) . 1_565 ?
O8 Ca3 O2 124.80(9) . 1_565 ?
O10 Ca3 O2 150.66(9) 2_564 1_565 ?
O10 Ca3 O2 107.86(9) 1_554 1_565 ?
O14 Ca3 O2 74.63(9) 1_556 1_565 ?
O12 Ca3 O2 85.27(8) 1_556 1_565 ?
O5 Ca3 O2 61.77(8) . 1_565 ?
O11 Ca3 Nb3 165.73(9) . . ?
O8 Ca3 Nb3 29.36(7) . . ?
O10 Ca3 Nb3 83.09(7) 2_564 . ?
O10 Ca3 Nb3 101.79(8) 1_554 . ?
O14 Ca3 Nb3 96.11(8) 1_556 . ?
O12 Ca3 Nb3 35.71(5) 1_556 . ?
O5 Ca3 Nb3 76.55(6) . . ?
O2 Ca3 Nb3 109.70(6) 1_565 . ?
O11 Ca3 Nb4 97.74(8) . 1_556 ?
O8 Ca3 Nb4 97.29(7) . 1_556 ?
O10 Ca3 Nb4 86.20(8) 2_564 1_556 ?
O10 Ca3 Nb4 170.05(8) 1_554 1_556 ?
O14 Ca3 Nb4 29.98(7) 1_556 1_556 ?
O12 Ca3 Nb4 34.50(5) 1_556 1_556 ?
O5 Ca3 Nb4 109.07(6) . 1_556 ?
O2 Ca3 Nb4 75.07(6) 1_565 1_556 ?
Nb3 Ca3 Nb4 68.41(3) . 1_556 ?
O11 Ca3 Nb3 85.65(8) . 1_554 ?
O8 Ca3 Nb3 82.57(7) . 1_554 ?
O10 Ca3 Nb3 124.67(8) 2_564 1_554 ?
O10 Ca3 Nb3 30.20(6) 1_554 1_554 ?
O14 Ca3 Nb3 150.86(8) 1_556 1_554 ?
O12 Ca3 Nb3 125.69(6) 1_556 1_554 ?
O5 Ca3 Nb3 40.70(6) . 1_554 ?
O2 Ca3 Nb3 78.93(6) 1_565 1_554 ?
Nb3 Ca3 Nb3 104.22(2) . 1_554 ?
Nb4 Ca3 Nb3 148.07(3) 1_556 1_554 ?
O11 Ca3 Nb4 28.38(7) . . ?
O8 Ca3 Nb4 147.18(7) . . ?
O10 Ca3 Nb4 127.92(8) 2_564 . ?
O10 Ca3 Nb4 85.34(8) 1_554 . ?
O14 Ca3 Nb4 84.66(8) 1_556 . ?
O12 Ca3 Nb4 123.35(6) 1_556 . ?
O5 Ca3 Nb4 78.27(6) . . ?
O2 Ca3 Nb4 39.58(6) 1_565 . ?
Nb3 Ca3 Nb4 147.95(3) . . ?
Nb4 Ca3 Nb4 102.08(2) 1_556 . ?
Nb3 Ca3 Nb4 67.03(3) 1_554 . ?
Nb4 O11 Ca3 113.49(13) . . ?
Nb4 O11 Ca4 103.63(12) . 1_556 ?
Ca3 O11 Ca4 108.84(13) . 1_556 ?
Nb4 O11 Ca4 98.39(13) . 2_575 ?
Ca3 O11 Ca4 127.40(12) . 2_575 ?
Ca4 O11 Ca4 102.32(11) 1_556 2_575 ?
Nb2 O4 Nb1 157.60(15) . 3_554 ?
Nb2 O4 Ca2 96.94(10) . 1_554 ?
Nb1 O4 Ca2 105.21(12) 3_554 1_554 ?
Nb2 O4 Ca1 91.11(11) . 3 ?
Nb1 O4 Ca1 88.13(9) 3_554 3 ?
Ca2 O4 Ca1 100.53(9) 1_554 3 ?
Nb2 O4 Ca1 90.63(10) . . ?
Nb1 O4 Ca1 83.22(9) 3_554 . ?
Ca2 O4 Ca1 97.75(10) 1_554 . ?
Ca1 O4 Ca1 161.28(12) 3 . ?
Nb2 O7 Nb3 137.63(15) . . ?
Nb2 O7 Ca1 104.87(12) . 1_556 ?
Nb3 O7 Ca1 110.08(12) . 1_556 ?
Nb2 O7 Ca2 98.95(11) . . ?
Nb3 O7 Ca2 93.10(10) . . ?
Ca1 O7 Ca2 107.01(11) 1_556 . ?
Nb1 O6 Nb2 156.64(15) 3 . ?
Nb1 O6 Ca2 97.33(11) 3 3_544 ?
Nb2 O6 Ca2 105.93(12) . 3_544 ?
Nb1 O6 Ca1 90.49(11) 3 1_556 ?
Nb2 O6 Ca1 87.66(9) . 1_556 ?
Ca2 O6 Ca1 100.05(10) 3_544 1_556 ?
Nb1 O6 Ca1 90.82(10) 3 3 ?
Nb2 O6 Ca1 83.87(9) . 3 ?
Ca2 O6 Ca1 98.06(11) 3_544 3 ?
Ca1 O6 Ca1 161.51(12) 1_556 3 ?
Nb3 O8 Ca4 140.94(15) . 1_546 ?
Nb3 O8 Ca3 108.91(13) . . ?
Ca4 O8 Ca3 108.86(12) 1_546 . ?
Nb1 O3 Nb2 158.90(18) . . ?
Nb1 O3 Ca1 100.14(12) . . ?
Nb2 O3 Ca1 100.68(11) . . ?
Nb1 O3 Ca2 90.89(9) . 3_544 ?
Nb2 O3 Ca2 91.95(9) . 3_544 ?
Ca1 O3 Ca2 91.60(9) . 3_544 ?
Nb1 O3 Ca1 80.08(10) . 1_556 ?
Nb2 O3 Ca1 80.12(10) . 1_556 ?
Ca1 O3 Ca1 169.26(11) . 1_556 ?
Ca2 O3 Ca1 77.66(7) 3_544 1_556 ?
Nb4 O14 Ca4 135.73(15) . . ?
Nb4 O14 Ca4 97.63(13) . 2_575 ?
Ca4 O14 Ca4 103.39(10) . 2_575 ?
Nb4 O14 Ca3 106.67(12) . 1_554 ?
Ca4 O14 Ca3 107.07(12) . 1_554 ?
Ca4 O14 Ca3 100.65(11) 2_575 1_554 ?
Nb3 O9 Nb4 143.07(16) . 1_546 ?
Nb3 O9 Ca4 96.63(11) . 1_547 ?
Nb4 O9 Ca4 96.70(10) 1_546 1_547 ?
Nb3 O9 Ca1 95.97(9) . 1_556 ?
Nb4 O9 Ca1 94.80(10) 1_546 1_556 ?
Ca4 O9 Ca1 141.27(12) 1_547 1_556 ?
Nb3 O10 Ca3 116.16(15) . 2_565 ?
Nb3 O10 Ca3 108.30(12) . 1_556 ?
Ca3 O10 Ca3 121.44(11) 2_565 1_556 ?
Nb3 O10 Ca4 101.81(12) . 1_547 ?
Ca3 O10 Ca4 103.16(11) 2_565 1_547 ?
Ca3 O10 Ca4 102.90(12) 1_556 1_547 ?
Nb1 O2 Nb4 149.33(16) . 1_545 ?
Nb1 O2 Ca2 94.17(11) . 1_544 ?
Nb4 O2 Ca2 85.68(10) 1_545 1_544 ?
Nb1 O2 Ca3 122.89(13) . 1_545 ?
Nb4 O2 Ca3 85.57(8) 1_545 1_545 ?
Ca2 O2 Ca3 109.05(10) 1_544 1_545 ?
Nb2 O5 Nb3 148.94(15) . 1_554 ?
Nb2 O5 Ca2 93.69(11) . 1_554 ?
Nb3 O5 Ca2 85.82(9) 1_554 1_554 ?
Nb2 O5 Ca3 122.87(13) . . ?
Nb3 O5 Ca3 85.69(8) 1_554 . ?
Ca2 O5 Ca3 110.94(10) 1_554 . ?
Nb1 O13 Nb4 140.16(14) 1_564 . ?
Nb1 O13 Ca1 103.88(12) 1_564 1_565 ?
Nb4 O13 Ca1 110.04(12) . 1_565 ?
Nb1 O13 Ca2 98.04(11) 1_564 1_554 ?
Nb4 O13 Ca2 92.13(10) . 1_554 ?
Ca1 O13 Ca2 106.17(11) 1_565 1_554 ?
Nb4 O12 Nb3 153.90(16) . 1_554 ?
Nb4 O12 Ca2 95.62(10) . 1_554 ?
Nb3 O12 Ca2 96.58(10) 1_554 1_554 ?
Nb4 O12 Ca3 96.18(10) . 1_554 ?
Nb3 O12 Ca3 93.30(10) 1_554 1_554 ?
Ca2 O12 Ca3 130.46(12) 1_554 1_554 ?
Nb1 O1 Nb2 141.82(16) . 1_545 ?
Nb1 O1 Ca2 103.11(12) . 1_545 ?
Nb2 O1 Ca2 102.22(12) 1_545 1_545 ?
Nb1 O1 Ca1 97.44(10) . 3_545 ?
Nb2 O1 Ca1 97.95(10) 1_545 3_545 ?
Ca2 O1 Ca1 113.74(12) 1_545 3_545 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O8 Nb3 Ca3 O11 -176.5(3) . . . . ?
O10 Nb3 Ca3 O11 89.7(3) . . . . ?
O9 Nb3 Ca3 O11 -160.9(3) . . . . ?
O12 Nb3 Ca3 O11 0.0(3) 1_556 . . . ?
O7 Nb3 Ca3 O11 -80.9(3) . . . . ?
O5 Nb3 Ca3 O11 -6.4(3) 1_556 . . . ?
Ca2 Nb3 Ca3 O11 -33.3(3) . . . . ?
Ca4 Nb3 Ca3 O11 119.5(3) 1_547 . . . ?
Ca3 Nb3 Ca3 O11 47.2(3) 1_556 . . . ?
Ca1 Nb3 Ca3 O11 -92.6(3) 1_556 . . . ?
Ca3 Nb3 Ca3 O11 114.3(3) 2_565 . . . ?
O10 Nb3 Ca3 O8 -93.79(16) . . . . ?
O9 Nb3 Ca3 O8 15.63(19) . . . . ?
O12 Nb3 Ca3 O8 176.45(17) 1_556 . . . ?
O7 Nb3 Ca3 O8 95.59(15) . . . . ?
O5 Nb3 Ca3 O8 170.10(16) 1_556 . . . ?
Ca2 Nb3 Ca3 O8 143.20(14) . . . . ?
Ca4 Nb3 Ca3 O8 -64.05(14) 1_547 . . . ?
Ca3 Nb3 Ca3 O8 -136.27(13) 1_556 . . . ?
Ca1 Nb3 Ca3 O8 83.91(14) 1_556 . . . ?
Ca3 Nb3 Ca3 O8 -69.25(13) 2_565 . . . ?
O8 Nb3 Ca3 O10 80.36(16) . . . 2_564 ?
O10 Nb3 Ca3 O10 -13.43(14) . . . 2_564 ?
O9 Nb3 Ca3 O10 95.99(15) . . . 2_564 ?
O12 Nb3 Ca3 O10 -103.18(12) 1_556 . . 2_564 ?
O7 Nb3 Ca3 O10 175.95(10) . . . 2_564 ?
O5 Nb3 Ca3 O10 -109.54(12) 1_556 . . 2_564 ?
Ca2 Nb3 Ca3 O10 -136.44(7) . . . 2_564 ?
Ca4 Nb3 Ca3 O10 16.31(9) 1_547 . . 2_564 ?
Ca3 Nb3 Ca3 O10 -55.91(8) 1_556 . . 2_564 ?
Ca1 Nb3 Ca3 O10 164.27(7) 1_556 . . 2_564 ?
Ca3 Nb3 Ca3 O10 11.11(7) 2_565 . . 2_564 ?
O8 Nb3 Ca3 O10 -12.81(14) . . . 1_554 ?
O10 Nb3 Ca3 O10 -106.60(12) . . . 1_554 ?
O9 Nb3 Ca3 O10 2.83(14) . . . 1_554 ?
O12 Nb3 Ca3 O10 163.65(12) 1_556 . . 1_554 ?
O7 Nb3 Ca3 O10 82.78(10) . . . 1_554 ?
O5 Nb3 Ca3 O10 157.29(11) 1_556 . . 1_554 ?
Ca2 Nb3 Ca3 O10 130.39(7) . . . 1_554 ?
Ca4 Nb3 Ca3 O10 -76.86(8) 1_547 . . 1_554 ?
Ca3 Nb3 Ca3 O10 -149.08(6) 1_556 . . 1_554 ?
Ca1 Nb3 Ca3 O10 71.10(7) 1_556 . . 1_554 ?
Ca3 Nb3 Ca3 O10 -82.06(7) 2_565 . . 1_554 ?
O8 Nb3 Ca3 O14 157.31(17) . . . 1_556 ?
O10 Nb3 Ca3 O14 63.52(12) . . . 1_556 ?
O9 Nb3 Ca3 O14 172.95(14) . . . 1_556 ?
O12 Nb3 Ca3 O14 -26.23(12) 1_556 . . 1_556 ?
O7 Nb3 Ca3 O14 -107.10(10) . . . 1_556 ?
O5 Nb3 Ca3 O14 -32.59(12) 1_556 . . 1_556 ?
Ca2 Nb3 Ca3 O14 -59.49(7) . . . 1_556 ?
Ca4 Nb3 Ca3 O14 93.26(8) 1_547 . . 1_556 ?
Ca3 Nb3 Ca3 O14 21.04(8) 1_556 . . 1_556 ?
Ca1 Nb3 Ca3 O14 -118.78(7) 1_556 . . 1_556 ?
Ca3 Nb3 Ca3 O14 88.06(7) 2_565 . . 1_556 ?
O8 Nb3 Ca3 O12 -176.45(17) . . . 1_556 ?
O10 Nb3 Ca3 O12 89.75(13) . . . 1_556 ?
O9 Nb3 Ca3 O12 -160.82(17) . . . 1_556 ?
O7 Nb3 Ca3 O12 -80.87(12) . . . 1_556 ?
O5 Nb3 Ca3 O12 -6.35(13) 1_556 . . 1_556 ?
Ca2 Nb3 Ca3 O12 -33.26(10) . . . 1_556 ?
Ca4 Nb3 Ca3 O12 119.50(11) 1_547 . . 1_556 ?
Ca3 Nb3 Ca3 O12 47.27(10) 1_556 . . 1_556 ?
Ca1 Nb3 Ca3 O12 -92.54(10) 1_556 . . 1_556 ?
Ca3 Nb3 Ca3 O12 114.29(10) 2_565 . . 1_556 ?
O8 Nb3 Ca3 O5 -73.88(14) . . . . ?
O10 Nb3 Ca3 O5 -167.67(11) . . . . ?
O9 Nb3 Ca3 O5 -58.25(14) . . . . ?
O12 Nb3 Ca3 O5 102.58(11) 1_556 . . . ?
O7 Nb3 Ca3 O5 21.71(9) . . . . ?
O5 Nb3 Ca3 O5 96.22(11) 1_556 . . . ?
Ca2 Nb3 Ca3 O5 69.32(6) . . . . ?
Ca4 Nb3 Ca3 O5 -137.93(7) 1_547 . . . ?
Ca3 Nb3 Ca3 O5 149.85(6) 1_556 . . . ?
Ca1 Nb3 Ca3 O5 10.03(6) 1_556 . . . ?
Ca3 Nb3 Ca3 O5 -143.13(6) 2_565 . . . ?
O8 Nb3 Ca3 O2 -126.85(15) . . . 1_565 ?
O10 Nb3 Ca3 O2 139.35(11) . . . 1_565 ?
O9 Nb3 Ca3 O2 -111.22(14) . . . 1_565 ?
O12 Nb3 Ca3 O2 49.60(12) 1_556 . . 1_565 ?
O7 Nb3 Ca3 O2 -31.27(10) . . . 1_565 ?
O5 Nb3 Ca3 O2 43.25(11) 1_556 . . 1_565 ?
Ca2 Nb3 Ca3 O2 16.34(7) . . . 1_565 ?
Ca4 Nb3 Ca3 O2 169.10(7) 1_547 . . 1_565 ?
Ca3 Nb3 Ca3 O2 96.88(7) 1_556 . . 1_565 ?
Ca1 Nb3 Ca3 O2 -42.94(7) 1_556 . . 1_565 ?
Ca3 Nb3 Ca3 O2 163.89(7) 2_565 . . 1_565 ?
O8 Nb3 Ca3 Nb4 169.00(13) . . . 1_556 ?
O10 Nb3 Ca3 Nb4 75.21(9) . . . 1_556 ?
O9 Nb3 Ca3 Nb4 -175.37(13) . . . 1_556 ?
O12 Nb3 Ca3 Nb4 -14.55(10) 1_556 . . 1_556 ?
O7 Nb3 Ca3 Nb4 -95.42(7) . . . 1_556 ?
O5 Nb3 Ca3 Nb4 -20.90(9) 1_556 . . 1_556 ?
Ca2 Nb3 Ca3 Nb4 -47.805(19) . . . 1_556 ?
Ca4 Nb3 Ca3 Nb4 104.95(4) 1_547 . . 1_556 ?
Ca3 Nb3 Ca3 Nb4 32.73(3) 1_556 . . 1_556 ?
Ca1 Nb3 Ca3 Nb4 -107.09(2) 1_556 . . 1_556 ?
Ca3 Nb3 Ca3 Nb4 99.743(17) 2_565 . . 1_556 ?
O8 Nb3 Ca3 Nb3 -43.73(13) . . . 1_554 ?
O10 Nb3 Ca3 Nb3 -137.52(9) . . . 1_554 ?
O9 Nb3 Ca3 Nb3 -28.10(13) . . . 1_554 ?
O12 Nb3 Ca3 Nb3 132.73(10) 1_556 . . 1_554 ?
O7 Nb3 Ca3 Nb3 51.86(8) . . . 1_554 ?
O5 Nb3 Ca3 Nb3 126.37(9) 1_556 . . 1_554 ?
Ca2 Nb3 Ca3 Nb3 99.47(3) . . . 1_554 ?
Ca4 Nb3 Ca3 Nb3 -107.78(4) 1_547 . . 1_554 ?
Ca3 Nb3 Ca3 Nb3 180.0 1_556 . . 1_554 ?
Ca1 Nb3 Ca3 Nb3 40.18(3) 1_556 . . 1_554 ?
Ca3 Nb3 Ca3 Nb3 -112.98(3) 2_565 . . 1_554 ?
O8 Nb3 Ca3 Nb4 -113.00(15) . . . . ?
O10 Nb3 Ca3 Nb4 153.21(11) . . . . ?
O9 Nb3 Ca3 Nb4 -97.36(13) . . . . ?
O12 Nb3 Ca3 Nb4 63.46(11) 1_556 . . . ?
O7 Nb3 Ca3 Nb4 -17.41(10) . . . . ?
O5 Nb3 Ca3 Nb4 57.10(12) 1_556 . . . ?
Ca2 Nb3 Ca3 Nb4 30.20(7) . . . . ?
Ca4 Nb3 Ca3 Nb4 -177.05(4) 1_547 . . . ?
Ca3 Nb3 Ca3 Nb4 110.73(6) 1_556 . . . ?
Ca1 Nb3 Ca3 Nb4 -29.09(8) 1_556 . . . ?
Ca3 Nb3 Ca3 Nb4 177.75(6) 2_565 . . . ?
O14 Nb4 Ca3 O11 -54.1(2) . . . . ?
O9 Nb4 Ca3 O11 64.85(18) 1_564 . . . ?
O12 Nb4 Ca3 O11 -132.79(18) . . . . ?
O13 Nb4 Ca3 O11 166.23(18) . . . . ?
O2 Nb4 Ca3 O11 131.62(18) 1_565 . . . ?
Ca4 Nb4 Ca3 O11 -30.81(16) 2_575 . . . ?
Ca2 Nb4 Ca3 O11 179.67(16) 1_554 . . . ?
Ca4 Nb4 Ca3 O11 41.54(16) 1_556 . . . ?
Ca3 Nb4 Ca3 O11 -96.11(16) 1_554 . . . ?
Ca1 Nb4 Ca3 O11 121.89(16) 1_565 . . . ?
O14 Nb4 Ca3 O8 97.19(17) . . . . ?
O11 Nb4 Ca3 O8 151.3(2) . . . . ?
O9 Nb4 Ca3 O8 -143.88(15) 1_564 . . . ?
O12 Nb4 Ca3 O8 18.49(16) . . . . ?
O13 Nb4 Ca3 O8 -42.49(17) . . . . ?
O2 Nb4 Ca3 O8 -77.10(16) 1_565 . . . ?
Ca4 Nb4 Ca3 O8 120.47(13) 2_575 . . . ?
Ca2 Nb4 Ca3 O8 -29.05(13) 1_554 . . . ?
Ca4 Nb4 Ca3 O8 -167.19(14) 1_556 . . . ?
Ca3 Nb4 Ca3 O8 55.16(14) 1_554 . . . ?
Ca1 Nb4 Ca3 O8 -86.84(14) 1_565 . . . ?
O14 Nb4 Ca3 O10 -43.34(14) . . . 2_564 ?
O11 Nb4 Ca3 O10 10.75(18) . . . 2_564 ?
O9 Nb4 Ca3 O10 75.60(13) 1_564 . . 2_564 ?
O12 Nb4 Ca3 O10 -122.04(13) . . . 2_564 ?
O13 Nb4 Ca3 O10 176.98(13) . . . 2_564 ?
O2 Nb4 Ca3 O10 142.37(13) 1_565 . . 2_564 ?
Ca4 Nb4 Ca3 O10 -20.06(10) 2_575 . . 2_564 ?
Ca2 Nb4 Ca3 O10 -169.58(10) 1_554 . . 2_564 ?
Ca4 Nb4 Ca3 O10 52.29(10) 1_556 . . 2_564 ?
Ca3 Nb4 Ca3 O10 -85.36(10) 1_554 . . 2_564 ?
Ca1 Nb4 Ca3 O10 132.64(10) 1_565 . . 2_564 ?
O14 Nb4 Ca3 O10 48.73(13) . . . 1_554 ?
O11 Nb4 Ca3 O10 102.82(18) . . . 1_554 ?
O9 Nb4 Ca3 O10 167.67(10) 1_564 . . 1_554 ?
O12 Nb4 Ca3 O10 -29.97(10) . . . 1_554 ?
O13 Nb4 Ca3 O10 -90.95(12) . . . 1_554 ?
O2 Nb4 Ca3 O10 -125.56(11) 1_565 . . 1_554 ?
Ca4 Nb4 Ca3 O10 72.01(7) 2_575 . . 1_554 ?
Ca2 Nb4 Ca3 O10 -77.51(7) 1_554 . . 1_554 ?
Ca4 Nb4 Ca3 O10 144.36(7) 1_556 . . 1_554 ?
Ca3 Nb4 Ca3 O10 6.71(7) 1_554 . . 1_554 ?
Ca1 Nb4 Ca3 O10 -135.29(7) 1_565 . . 1_554 ?
O14 Nb4 Ca3 O14 -113.45(14) . . . 1_556 ?
O11 Nb4 Ca3 O14 -59.36(17) . . . 1_556 ?
O9 Nb4 Ca3 O14 5.49(11) 1_564 . . 1_556 ?
O12 Nb4 Ca3 O14 167.86(10) . . . 1_556 ?
O13 Nb4 Ca3 O14 106.88(12) . . . 1_556 ?
O2 Nb4 Ca3 O14 72.26(11) 1_565 . . 1_556 ?
Ca4 Nb4 Ca3 O14 -90.17(7) 2_575 . . 1_556 ?
Ca2 Nb4 Ca3 O14 120.31(7) 1_554 . . 1_556 ?
Ca4 Nb4 Ca3 O14 -17.82(7) 1_556 . . 1_556 ?
Ca3 Nb4 Ca3 O14 -155.47(6) 1_554 . . 1_556 ?
Ca1 Nb4 Ca3 O14 62.53(7) 1_565 . . 1_556 ?
O14 Nb4 Ca3 O12 -167.74(12) . . . 1_556 ?
O11 Nb4 Ca3 O12 -113.65(18) . . . 1_556 ?
O9 Nb4 Ca3 O12 -48.81(10) 1_564 . . 1_556 ?
O12 Nb4 Ca3 O12 113.56(12) . . . 1_556 ?
O13 Nb4 Ca3 O12 52.58(12) . . . 1_556 ?
O2 Nb4 Ca3 O12 17.97(11) 1_565 . . 1_556 ?
Ca4 Nb4 Ca3 O12 -144.46(7) 2_575 . . 1_556 ?
Ca2 Nb4 Ca3 O12 66.02(7) 1_554 . . 1_556 ?
Ca4 Nb4 Ca3 O12 -72.12(7) 1_556 . . 1_556 ?
Ca3 Nb4 Ca3 O12 150.23(7) 1_554 . . 1_556 ?
Ca1 Nb4 Ca3 O12 8.23(8) 1_565 . . 1_556 ?
O14 Nb4 Ca3 O5 114.76(12) . . . . ?
O11 Nb4 Ca3 O5 168.84(17) . . . . ?
O9 Nb4 Ca3 O5 -126.31(10) 1_564 . . . ?
O12 Nb4 Ca3 O5 36.06(10) . . . . ?
O13 Nb4 Ca3 O5 -24.92(11) . . . . ?
O2 Nb4 Ca3 O5 -59.53(11) 1_565 . . . ?
Ca4 Nb4 Ca3 O5 138.04(6) 2_575 . . . ?
Ca2 Nb4 Ca3 O5 -11.48(6) 1_554 . . . ?
Ca4 Nb4 Ca3 O5 -149.62(6) 1_556 . . . ?
Ca3 Nb4 Ca3 O5 72.73(6) 1_554 . . . ?
Ca1 Nb4 Ca3 O5 -69.27(6) 1_565 . . . ?
O14 Nb4 Ca3 O2 174.29(14) . . . 1_565 ?
O11 Nb4 Ca3 O2 -131.62(18) . . . 1_565 ?
O9 Nb4 Ca3 O2 -66.78(12) 1_564 . . 1_565 ?
O12 Nb4 Ca3 O2 95.59(12) . . . 1_565 ?
O13 Nb4 Ca3 O2 34.61(13) . . . 1_565 ?
Ca4 Nb4 Ca3 O2 -162.43(9) 2_575 . . 1_565 ?
Ca2 Nb4 Ca3 O2 48.05(9) 1_554 . . 1_565 ?
Ca4 Nb4 Ca3 O2 -90.08(9) 1_556 . . 1_565 ?
Ca3 Nb4 Ca3 O2 132.27(9) 1_554 . . 1_565 ?
Ca1 Nb4 Ca3 O2 -9.74(9) 1_565 . . 1_565 ?
O14 Nb4 Ca3 Nb3 153.56(11) . . . . ?
O11 Nb4 Ca3 Nb3 -152.35(18) . . . . ?
O9 Nb4 Ca3 Nb3 -87.50(10) 1_564 . . . ?
O12 Nb4 Ca3 Nb3 74.87(10) . . . . ?
O13 Nb4 Ca3 Nb3 13.89(13) . . . . ?
O2 Nb4 Ca3 Nb3 -20.72(11) 1_565 . . . ?
Ca4 Nb4 Ca3 Nb3 176.84(6) 2_575 . . . ?
Ca2 Nb4 Ca3 Nb3 27.32(6) 1_554 . . . ?
Ca4 Nb4 Ca3 Nb3 -110.81(6) 1_556 . . . ?
Ca3 Nb4 Ca3 Nb3 111.54(6) 1_554 . . . ?
Ca1 Nb4 Ca3 Nb3 -30.46(7) 1_565 . . . ?
O14 Nb4 Ca3 Nb4 -137.98(11) . . . 1_556 ?
O11 Nb4 Ca3 Nb4 -83.89(16) . . . 1_556 ?
O9 Nb4 Ca3 Nb4 -19.04(8) 1_564 . . 1_556 ?
O12 Nb4 Ca3 Nb4 143.32(8) . . . 1_556 ?
O13 Nb4 Ca3 Nb4 82.34(10) . . . 1_556 ?
O2 Nb4 Ca3 Nb4 47.73(9) 1_565 . . 1_556 ?
Ca4 Nb4 Ca3 Nb4 -114.70(2) 2_575 . . 1_556 ?
Ca2 Nb4 Ca3 Nb4 95.78(2) 1_554 . . 1_556 ?
Ca4 Nb4 Ca3 Nb4 -42.35(2) 1_556 . . 1_556 ?
Ca3 Nb4 Ca3 Nb4 180.0 1_554 . . 1_556 ?
Ca1 Nb4 Ca3 Nb4 38.00(3) 1_565 . . 1_556 ?
O14 Nb4 Ca3 Nb3 73.60(11) . . . 1_554 ?
O11 Nb4 Ca3 Nb3 127.69(16) . . . 1_554 ?
O9 Nb4 Ca3 Nb3 -167.46(8) 1_564 . . 1_554 ?
O12 Nb4 Ca3 Nb3 -5.10(8) . . . 1_554 ?
O13 Nb4 Ca3 Nb3 -66.07(10) . . . 1_554 ?
O2 Nb4 Ca3 Nb3 -100.69(9) 1_565 . . 1_554 ?
Ca4 Nb4 Ca3 Nb3 96.882(19) 2_575 . . 1_554 ?
Ca2 Nb4 Ca3 Nb3 -52.638(19) 1_554 . . 1_554 ?
Ca4 Nb4 Ca3 Nb3 169.23(2) 1_556 . . 1_554 ?
Ca3 Nb4 Ca3 Nb3 31.58(3) 1_554 . . 1_554 ?
Ca1 Nb4 Ca3 Nb3 -110.42(2) 1_565 . . 1_554 ?
O14 Nb4 O11 Ca3 136.27(15) . . . . ?
O9 Nb4 O11 Ca3 -122.01(15) 1_564 . . . ?
O12 Nb4 O11 Ca3 43.28(16) . . . . ?
O13 Nb4 O11 Ca3 -41.9(5) . . . . ?
O2 Nb4 O11 Ca3 -37.99(14) 1_565 . . . ?
Ca4 Nb4 O11 Ca3 137.2(2) 2_575 . . . ?
Ca2 Nb4 O11 Ca3 -0.37(18) 1_554 . . . ?
Ca4 Nb4 O11 Ca3 -117.88(19) 1_556 . . . ?
Ca3 Nb4 O11 Ca3 92.79(13) 1_554 . . . ?
Ca1 Nb4 O11 Ca3 -86.23(15) 1_565 . . . ?
O14 Nb4 O11 Ca4 -105.86(14) . . . 1_556 ?
O9 Nb4 O11 Ca4 -4.14(12) 1_564 . . 1_556 ?
O12 Nb4 O11 Ca4 161.16(12) . . . 1_556 ?
O13 Nb4 O11 Ca4 76.0(4) . . . 1_556 ?
O2 Nb4 O11 Ca4 79.89(12) 1_565 . . 1_556 ?
Ca4 Nb4 O11 Ca4 -104.94(14) 2_575 . . 1_556 ?
Ca2 Nb4 O11 Ca4 117.50(9) 1_554 . . 1_556 ?
Ca3 Nb4 O11 Ca4 -149.33(8) 1_554 . . 1_556 ?
Ca3 Nb4 O11 Ca4 117.88(19) . . . 1_556 ?
Ca1 Nb4 O11 Ca4 31.65(17) 1_565 . . 1_556 ?
O14 Nb4 O11 Ca4 -0.92(12) . . . 2_575 ?
O9 Nb4 O11 Ca4 100.80(12) 1_564 . . 2_575 ?
O12 Nb4 O11 Ca4 -93.90(12) . . . 2_575 ?
O13 Nb4 O11 Ca4 -179.0(3) . . . 2_575 ?
O2 Nb4 O11 Ca4 -175.18(12) 1_565 . . 2_575 ?
Ca2 Nb4 O11 Ca4 -137.56(6) 1_554 . . 2_575 ?
Ca4 Nb4 O11 Ca4 104.94(14) 1_556 . . 2_575 ?
Ca3 Nb4 O11 Ca4 -44.40(10) 1_554 . . 2_575 ?
Ca3 Nb4 O11 Ca4 -137.2(2) . . . 2_575 ?
Ca1 Nb4 O11 Ca4 136.59(7) 1_565 . . 2_575 ?
O8 Ca3 O11 Nb4 -85.9(4) . . . . ?
O10 Ca3 O11 Nb4 -171.41(14) 2_564 . . . ?
O10 Ca3 O11 Nb4 -76.51(16) 1_554 . . . ?
O14 Ca3 O11 Nb4 115.15(16) 1_556 . . . ?
O12 Ca3 O11 Nb4 87.49(18) 1_556 . . . ?
O5 Ca3 O11 Nb4 -11.37(17) . . . . ?
O2 Ca3 O11 Nb4 32.81(13) 1_565 . . . ?
Nb3 Ca3 O11 Nb4 87.5(3) . . . . ?
Nb4 Ca3 O11 Nb4 101.12(14) 1_556 . . . ?
Nb3 Ca3 O11 Nb4 -46.94(14) 1_554 . . . ?
O8 Ca3 O11 Ca4 159.3(3) . . . 1_556 ?
O10 Ca3 O11 Ca4 73.78(12) 2_564 . . 1_556 ?
O10 Ca3 O11 Ca4 168.68(9) 1_554 . . 1_556 ?
O14 Ca3 O11 Ca4 0.34(10) 1_556 . . 1_556 ?
O12 Ca3 O11 Ca4 -27.32(17) 1_556 . . 1_556 ?
O5 Ca3 O11 Ca4 -126.18(11) . . . 1_556 ?
O2 Ca3 O11 Ca4 -82.00(11) 1_565 . . 1_556 ?
Nb3 Ca3 O11 Ca4 -27.3(4) . . . 1_556 ?
Nb4 Ca3 O11 Ca4 -13.69(10) 1_556 . . 1_556 ?
Nb3 Ca3 O11 Ca4 -161.75(10) 1_554 . . 1_556 ?
Nb4 Ca3 O11 Ca4 -114.81(19) . . . 1_556 ?
O8 Ca3 O11 Ca4 36.3(5) . . . 2_575 ?
O10 Ca3 O11 Ca4 -49.22(19) 2_564 . . 2_575 ?
O10 Ca3 O11 Ca4 45.68(18) 1_554 . . 2_575 ?
O14 Ca3 O11 Ca4 -122.66(18) 1_556 . . 2_575 ?
O12 Ca3 O11 Ca4 -150.32(13) 1_556 . . 2_575 ?
O5 Ca3 O11 Ca4 110.81(15) . . . 2_575 ?
O2 Ca3 O11 Ca4 155.00(19) 1_565 . . 2_575 ?
Nb3 Ca3 O11 Ca4 -150.3(2) . . . 2_575 ?
Nb4 Ca3 O11 Ca4 -136.70(14) 1_556 . . 2_575 ?
Nb3 Ca3 O11 Ca4 75.24(15) 1_554 . . 2_575 ?
Nb4 Ca3 O11 Ca4 122.2(3) . . . 2_575 ?
O5 Nb2 O4 Nb1 -143.6(4) . . . 3_554 ?
O7 Nb2 O4 Nb1 56.2(6) . . . 3_554 ?
O3 Nb2 O4 Nb1 -44.2(4) . . . 3_554 ?
O1 Nb2 O4 Nb1 121.1(4) 1_565 . . 3_554 ?
O6 Nb2 O4 Nb1 40.4(4) . . . 3_554 ?
Ca2 Nb2 O4 Nb1 -171.4(5) 1_554 . . 3_554 ?
Ca1 Nb2 O4 Nb1 87.8(4) 3 . . 3_554 ?
Ca2 Nb2 O4 Nb1 100.7(4) . . . 3_554 ?
Ca1 Nb2 O4 Nb1 11.1(4) 1_556 . . 3_554 ?
Ca1 Nb2 O4 Nb1 -73.6(4) . . . 3_554 ?
Ca2 Nb2 O4 Nb1 7.4(3) 3_544 . . 3_554 ?
O5 Nb2 O4 Ca2 27.85(12) . . . 1_554 ?
O7 Nb2 O4 Ca2 -132.3(4) . . . 1_554 ?
O3 Nb2 O4 Ca2 127.28(11) . . . 1_554 ?
O1 Nb2 O4 Ca2 -67.41(11) 1_565 . . 1_554 ?
O6 Nb2 O4 Ca2 -148.17(11) . . . 1_554 ?
Ca1 Nb2 O4 Ca2 -100.75(10) 3 . . 1_554 ?
Ca2 Nb2 O4 Ca2 -87.90(10) . . . 1_554 ?
Ca1 Nb2 O4 Ca2 -177.41(4) 1_556 . . 1_554 ?
Ca1 Nb2 O4 Ca2 97.89(11) . . . 1_554 ?
Ca2 Nb2 O4 Ca2 178.88(12) 3_544 . . 1_554 ?
O5 Nb2 O4 Ca1 128.60(10) . . . 3 ?
O7 Nb2 O4 Ca1 -31.6(4) . . . 3 ?
O3 Nb2 O4 Ca1 -131.97(10) . . . 3 ?
O1 Nb2 O4 Ca1 33.34(10) 1_565 . . 3 ?
O6 Nb2 O4 Ca1 -47.42(9) . . . 3 ?
Ca2 Nb2 O4 Ca1 100.75(10) 1_554 . . 3 ?
Ca2 Nb2 O4 Ca1 12.85(11) . . . 3 ?
Ca1 Nb2 O4 Ca1 -76.66(9) 1_556 . . 3 ?
Ca1 Nb2 O4 Ca1 -161.36(12) . . . 3 ?
Ca2 Nb2 O4 Ca1 -80.37(8) 3_544 . . 3 ?
O5 Nb2 O4 Ca1 -70.04(11) . . . . ?
O7 Nb2 O4 Ca1 129.8(4) . . . . ?
O3 Nb2 O4 Ca1 29.40(10) . . . . ?
O1 Nb2 O4 Ca1 -165.30(10) 1_565 . . . ?
O6 Nb2 O4 Ca1 113.94(9) . . . . ?
Ca2 Nb2 O4 Ca1 -97.89(11) 1_554 . . . ?
Ca1 Nb2 O4 Ca1 161.36(12) 3 . . . ?
Ca2 Nb2 O4 Ca1 174.21(3) . . . . ?
Ca1 Nb2 O4 Ca1 84.70(10) 1_556 . . . ?
Ca2 Nb2 O4 Ca1 80.99(6) 3_544 . . . ?
O7 Ca1 O4 Nb2 96.38(11) 1_554 . . . ?
O13 Ca1 O4 Nb2 51.3(6) 1_545 . . . ?
O1 Ca1 O4 Nb2 -121.22(13) 3_554 . . . ?
O3 Ca1 O4 Nb2 -26.51(9) . . . . ?
O4 Ca1 O4 Nb2 -147.34(10) 3_544 . . . ?
O6 Ca1 O4 Nb2 165.37(12) 1_554 . . . ?
O6 Ca1 O4 Nb2 -74.35(11) 3_544 . . . ?
O9 Ca1 O4 Nb2 38.75(11) 1_554 . . . ?
O3 Ca1 O4 Nb2 142.25(8) 1_554 . . . ?
Nb1 Ca1 O4 Nb2 -158.40(15) 3_554 . . . ?
Nb2 Ca1 O4 Nb2 -116.88(8) 3_544 . . . ?
O7 Ca1 O4 Nb1 -105.22(10) 1_554 . . 3_554 ?
O13 Ca1 O4 Nb1 -150.3(5) 1_545 . . 3_554 ?
O1 Ca1 O4 Nb1 37.19(10) 3_554 . . 3_554 ?
O3 Ca1 O4 Nb1 131.89(11) . . . 3_554 ?
O4 Ca1 O4 Nb1 11.06(19) 3_544 . . 3_554 ?
O6 Ca1 O4 Nb1 -36.23(9) 1_554 . . 3_554 ?
O6 Ca1 O4 Nb1 84.05(11) 3_544 . . 3_554 ?
O9 Ca1 O4 Nb1 -162.85(8) 1_554 . . 3_554 ?
O3 Ca1 O4 Nb1 -59.35(10) 1_554 . . 3_554 ?
Nb2 Ca1 O4 Nb1 41.52(8) 3_544 . . 3_554 ?
O7 Ca1 O4 Ca2 -0.71(10) 1_554 . . 1_554 ?
O13 Ca1 O4 Ca2 -45.8(6) 1_545 . . 1_554 ?
O1 Ca1 O4 Ca2 141.69(13) 3_554 . . 1_554 ?
O3 Ca1 O4 Ca2 -123.60(11) . . . 1_554 ?
O4 Ca1 O4 Ca2 115.57(9) 3_544 . . 1_554 ?
O6 Ca1 O4 Ca2 68.28(9) 1_554 . . 1_554 ?
O6 Ca1 O4 Ca2 -171.44(8) 3_544 . . 1_554 ?
O9 Ca1 O4 Ca2 -58.34(11) 1_554 . . 1_554 ?
O3 Ca1 O4 Ca2 45.16(12) 1_554 . . 1_554 ?
Nb1 Ca1 O4 Ca2 104.51(12) 3_554 . . 1_554 ?
Nb2 Ca1 O4 Ca2 146.02(7) 3_544 . . 1_554 ?
O7 Ca1 O4 Ca1 -168.3(4) 1_554 . . 3 ?
O13 Ca1 O4 Ca1 146.7(4) 1_545 . . 3 ?
O1 Ca1 O4 Ca1 -25.9(4) 3_554 . . 3 ?
O3 Ca1 O4 Ca1 68.8(4) . . . 3 ?
O4 Ca1 O4 Ca1 -52.0(5) 3_544 . . 3 ?
O6 Ca1 O4 Ca1 -99.3(4) 1_554 . . 3 ?
O6 Ca1 O4 Ca1 21.0(4) 3_544 . . 3 ?
O9 Ca1 O4 Ca1 134.1(4) 1_554 . . 3 ?
O3 Ca1 O4 Ca1 -122.4(4) 1_554 . . 3 ?
Nb1 Ca1 O4 Ca1 -63.1(4) 3_554 . . 3 ?
Nb2 Ca1 O4 Ca1 -21.5(4) 3_544 . . 3 ?
O5 Nb2 O7 Nb3 -1.2(2) . . . . ?
O3 Nb2 O7 Nb3 -101.9(2) . . . . ?
O4 Nb2 O7 Nb3 158.5(3) . . . . ?
O1 Nb2 O7 Nb3 93.8(2) 1_565 . . . ?
O6 Nb2 O7 Nb3 174.5(2) . . . . ?
Ca2 Nb2 O7 Nb3 40.5(3) 1_554 . . . ?
Ca1 Nb2 O7 Nb3 131.51(17) 3 . . . ?
Ca2 Nb2 O7 Nb3 104.7(2) . . . . ?
Ca1 Nb2 O7 Nb3 -144.9(3) 1_556 . . . ?
Ca1 Nb2 O7 Nb3 -82.9(2) . . . . ?
Ca2 Nb2 O7 Nb3 -157.26(17) 3_544 . . . ?
O5 Nb2 O7 Ca1 143.70(12) . . . 1_556 ?
O3 Nb2 O7 Ca1 43.02(12) . . . 1_556 ?
O4 Nb2 O7 Ca1 -56.6(4) . . . 1_556 ?
O1 Nb2 O7 Ca1 -121.29(12) 1_565 . . 1_556 ?
O6 Nb2 O7 Ca1 -40.55(11) . . . 1_556 ?
Ca2 Nb2 O7 Ca1 -174.57(4) 1_554 . . 1_556 ?
Ca1 Nb2 O7 Ca1 -83.58(10) 3 . . 1_556 ?
Ca2 Nb2 O7 Ca1 -110.38(14) . . . 1_556 ?
Ca1 Nb2 O7 Ca1 62.01(15) . . . 1_556 ?
Ca2 Nb2 O7 Ca1 -12.35(12) 3_544 . . 1_556 ?
O5 Nb2 O7 Ca2 -105.92(12) . . . . ?
O3 Nb2 O7 Ca2 153.39(11) . . . . ?
O4 Nb2 O7 Ca2 53.8(4) . . . . ?
O1 Nb2 O7 Ca2 -10.91(10) 1_565 . . . ?
O6 Nb2 O7 Ca2 69.82(10) . . . . ?
Ca2 Nb2 O7 Ca2 -64.19(16) 1_554 . . . ?
Ca1 Nb2 O7 Ca2 26.79(11) 3 . . . ?
Ca1 Nb2 O7 Ca2 110.38(14) 1_556 . . . ?
Ca1 Nb2 O7 Ca2 172.38(4) . . . . ?
Ca2 Nb2 O7 Ca2 98.02(8) 3_544 . . . ?
O8 Nb3 O7 Nb2 21.6(2) . . . . ?
O10 Nb3 O7 Nb2 -156.7(4) . . . . ?
O9 Nb3 O7 Nb2 123.3(2) . . . . ?
O12 Nb3 O7 Nb2 -70.7(2) 1_556 . . . ?
O5 Nb3 O7 Nb2 -152.7(2) 1_556 . . . ?
Ca2 Nb3 O7 Nb2 -106.9(2) . . . . ?
Ca4 Nb3 O7 Nb2 143.21(15) 1_547 . . . ?
Ca3 Nb3 O7 Nb2 -19.91(19) . . . . ?
Ca3 Nb3 O7 Nb2 -126.72(17) 1_556 . . . ?
Ca1 Nb3 O7 Nb2 143.7(3) 1_556 . . . ?
Ca3 Nb3 O7 Nb2 19.8(3) 2_565 . . . ?
O8 Nb3 O7 Ca1 -122.09(14) . . . 1_556 ?
O10 Nb3 O7 Ca1 59.6(5) . . . 1_556 ?
O9 Nb3 O7 Ca1 -20.48(13) . . . 1_556 ?
O12 Nb3 O7 Ca1 145.58(14) 1_556 . . 1_556 ?
O5 Nb3 O7 Ca1 63.60(12) 1_556 . . 1_556 ?
Ca2 Nb3 O7 Ca1 109.37(15) . . . 1_556 ?
Ca4 Nb3 O7 Ca1 -0.52(16) 1_547 . . 1_556 ?
Ca3 Nb3 O7 Ca1 -163.64(11) . . . 1_556 ?
Ca3 Nb3 O7 Ca1 89.55(12) 1_556 . . 1_556 ?
Ca3 Nb3 O7 Ca1 -123.96(14) 2_565 . . 1_556 ?
O8 Nb3 O7 Ca2 128.54(11) . . . . ?
O10 Nb3 O7 Ca2 -49.8(5) . . . . ?
O9 Nb3 O7 Ca2 -129.85(12) . . . . ?
O12 Nb3 O7 Ca2 36.21(12) 1_556 . . . ?
O5 Nb3 O7 Ca2 -45.77(9) 1_556 . . . ?
Ca4 Nb3 O7 Ca2 -109.89(8) 1_547 . . . ?
Ca3 Nb3 O7 Ca2 86.99(7) . . . . ?
Ca3 Nb3 O7 Ca2 -19.82(12) 1_556 . . . ?
Ca1 Nb3 O7 Ca2 -109.37(15) 1_556 . . . ?
Ca3 Nb3 O7 Ca2 126.67(14) 2_565 . . . ?
O1 Ca2 O7 Nb2 10.08(9) 1_565 . . . ?
O4 Ca2 O7 Nb2 -109.45(12) 1_556 . . . ?
O6 Ca2 O7 Nb2 -88.5(4) 3 . . . ?
O12 Ca2 O7 Nb2 107.90(12) 1_556 . . . ?
O13 Ca2 O7 Nb2 62.43(14) 1_556 . . . ?
O2 Ca2 O7 Nb2 142.08(11) 1_566 . . . ?
O5 Ca2 O7 Nb2 -178.54(13) 1_556 . . . ?
O3 Ca2 O7 Nb2 -52.85(12) 3 . . . ?
Nb2 Ca2 O7 Nb2 -146.68(10) 1_556 . . . ?
Nb1 Ca2 O7 Nb2 -178.59(5) 1_566 . . . ?
Nb4 Ca2 O7 Nb2 101.49(9) 1_556 . . . ?
O1 Ca2 O7 Nb3 -129.17(12) 1_565 . . . ?
O4 Ca2 O7 Nb3 111.29(11) 1_556 . . . ?
O6 Ca2 O7 Nb3 132.2(3) 3 . . . ?
O12 Ca2 O7 Nb3 -31.35(10) 1_556 . . . ?
O13 Ca2 O7 Nb3 -76.83(13) 1_556 . . . ?
O2 Ca2 O7 Nb3 2.82(15) 1_566 . . . ?
O5 Ca2 O7 Nb3 42.21(9) 1_556 . . . ?
O3 Ca2 O7 Nb3 167.90(9) 3 . . . ?
Nb2 Ca2 O7 Nb3 74.07(8) 1_556 . . . ?
Nb1 Ca2 O7 Nb3 42.15(17) 1_566 . . . ?
Nb4 Ca2 O7 Nb3 -37.76(9) 1_556 . . . ?
O1 Ca2 O7 Ca1 118.73(13) 1_565 . . 1_556 ?
O4 Ca2 O7 Ca1 -0.80(11) 1_556 . . 1_556 ?
O6 Ca2 O7 Ca1 20.1(4) 3 . . 1_556 ?
O12 Ca2 O7 Ca1 -143.44(14) 1_556 . . 1_556 ?
O13 Ca2 O7 Ca1 171.08(8) 1_556 . . 1_556 ?
O2 Ca2 O7 Ca1 -109.27(12) 1_566 . . 1_556 ?
O5 Ca2 O7 Ca1 -69.88(11) 1_556 . . 1_556 ?
O3 Ca2 O7 Ca1 55.81(12) 3 . . 1_556 ?
Nb2 Ca2 O7 Ca1 -38.03(9) 1_556 . . 1_556 ?
Nb1 Ca2 O7 Ca1 -69.94(16) 1_566 . . 1_556 ?
Nb4 Ca2 O7 Ca1 -149.85(8) 1_556 . . 1_556 ?
O5 Nb2 O6 Nb1 65.9(16) . . . 3 ?
O7 Nb2 O6 Nb1 -52.2(4) . . . 3 ?
O3 Nb2 O6 Nb1 -147.5(4) . . . 3 ?
O4 Nb2 O6 Nb1 123.6(4) . . . 3 ?
O1 Nb2 O6 Nb1 37.0(4) 1_565 . . 3 ?
Ca2 Nb2 O6 Nb1 96.4(4) 1_554 . . 3 ?
Ca1 Nb2 O6 Nb1 77.7(4) 3 . . 3 ?
Ca2 Nb2 O6 Nb1 -5.1(4) . . . 3 ?
Ca1 Nb2 O6 Nb1 -85.8(4) 1_556 . . 3 ?
Ca1 Nb2 O6 Nb1 173.4(4) . . . 3 ?
Ca2 Nb2 O6 Nb1 174.4(5) 3_544 . . 3 ?
O5 Nb2 O6 Ca2 -108.5(14) . . . 3_544 ?
O7 Nb2 O6 Ca2 133.41(13) . . . 3_544 ?
O3 Nb2 O6 Ca2 38.07(12) . . . 3_544 ?
O4 Nb2 O6 Ca2 -50.84(11) . . . 3_544 ?
O1 Nb2 O6 Ca2 -137.37(13) 1_565 . . 3_544 ?
Ca2 Nb2 O6 Ca2 -78.04(11) 1_554 . . 3_544 ?
Ca1 Nb2 O6 Ca2 -96.66(12) 3 . . 3_544 ?
Ca2 Nb2 O6 Ca2 -179.54(12) . . . 3_544 ?
Ca1 Nb2 O6 Ca2 99.79(11) 1_556 . . 3_544 ?
Ca1 Nb2 O6 Ca2 -0.98(11) . . . 3_544 ?
O5 Nb2 O6 Ca1 151.7(14) . . . 1_556 ?
O7 Nb2 O6 Ca1 33.62(9) . . . 1_556 ?
O3 Nb2 O6 Ca1 -61.72(10) . . . 1_556 ?
O4 Nb2 O6 Ca1 -150.63(10) . . . 1_556 ?
O1 Nb2 O6 Ca1 122.85(11) 1_565 . . 1_556 ?
Ca2 Nb2 O6 Ca1 -177.83(3) 1_554 . . 1_556 ?
Ca1 Nb2 O6 Ca1 163.55(12) 3 . . 1_556 ?
Ca2 Nb2 O6 Ca1 80.67(7) . . . 1_556 ?
Ca1 Nb2 O6 Ca1 -100.77(7) . . . 1_556 ?
Ca2 Nb2 O6 Ca1 -99.79(11) 3_544 . . 1_556 ?
O5 Nb2 O6 Ca1 -11.8(14) . . . 3 ?
O7 Nb2 O6 Ca1 -129.92(10) . . . 3 ?
O3 Nb2 O6 Ca1 134.73(11) . . . 3 ?
O4 Nb2 O6 Ca1 45.82(9) . . . 3 ?
O1 Nb2 O6 Ca1 -40.70(10) 1_565 . . 3 ?
Ca2 Nb2 O6 Ca1 18.62(10) 1_554 . . 3 ?
Ca2 Nb2 O6 Ca1 -82.88(6) . . . 3 ?
Ca1 Nb2 O6 Ca1 -163.55(12) 1_556 . . 3 ?
Ca1 Nb2 O6 Ca1 95.68(6) . . . 3 ?
Ca2 Nb2 O6 Ca1 96.66(12) 3_544 . . 3 ?
O10 Nb3 O8 Ca4 -100.6(2) . . . 1_546 ?
O9 Nb3 O8 Ca4 -5.8(3) . . . 1_546 ?
O12 Nb3 O8 Ca4 161.9(2) 1_556 . . 1_546 ?
O7 Nb3 O8 Ca4 79.8(2) . . . 1_546 ?
O5 Nb3 O8 Ca4 115.0(6) 1_556 . . 1_546 ?
Ca2 Nb3 O8 Ca4 121.3(2) . . . 1_546 ?
Ca4 Nb3 O8 Ca4 -54.5(2) 1_547 . . 1_546 ?
Ca3 Nb3 O8 Ca4 164.6(3) . . . 1_546 ?
Ca3 Nb3 O8 Ca4 -133.56(18) 1_556 . . 1_546 ?
Ca1 Nb3 O8 Ca4 46.9(2) 1_556 . . 1_546 ?
Ca3 Nb3 O8 Ca4 -101.0(2) 2_565 . . 1_546 ?
O10 Nb3 O8 Ca3 94.74(13) . . . . ?
O9 Nb3 O8 Ca3 -170.39(12) . . . . ?
O12 Nb3 O8 Ca3 -2.76(13) 1_556 . . . ?
O7 Nb3 O8 Ca3 -84.86(12) . . . . ?
O5 Nb3 O8 Ca3 -49.6(7) 1_556 . . . ?
Ca2 Nb3 O8 Ca3 -43.34(14) . . . . ?
Ca4 Nb3 O8 Ca3 140.89(8) 1_547 . . . ?
Ca3 Nb3 O8 Ca3 61.80(15) 1_556 . . . ?
Ca1 Nb3 O8 Ca3 -117.68(9) 1_556 . . . ?
Ca3 Nb3 O8 Ca3 94.32(11) 2_565 . . . ?
O11 Ca3 O8 Nb3 176.7(3) . . . . ?
O10 Ca3 O8 Nb3 -95.02(15) 2_564 . . . ?
O10 Ca3 O8 Nb3 166.89(15) 1_554 . . . ?
O14 Ca3 O8 Nb3 -27.16(19) 1_556 . . . ?
O12 Ca3 O8 Nb3 2.28(11) 1_556 . . . ?
O5 Ca3 O8 Nb3 97.40(13) . . . . ?
O2 Ca3 O8 Nb3 66.55(16) 1_565 . . . ?
Nb4 Ca3 O8 Nb3 -10.31(13) 1_556 . . . ?
Nb3 Ca3 O8 Nb3 137.49(12) 1_554 . . . ?
Nb4 Ca3 O8 Nb3 115.68(13) . . . . ?
O11 Ca3 O8 Ca4 6.9(4) . . . 1_546 ?
O10 Ca3 O8 Ca4 95.15(12) 2_564 . . 1_546 ?
O10 Ca3 O8 Ca4 -2.94(10) 1_554 . . 1_546 ?
O14 Ca3 O8 Ca4 163.00(9) 1_556 . . 1_546 ?
O12 Ca3 O8 Ca4 -167.55(14) 1_556 . . 1_546 ?
O5 Ca3 O8 Ca4 -72.43(11) . . . 1_546 ?
O2 Ca3 O8 Ca4 -103.29(12) 1_565 . . 1_546 ?
Nb3 Ca3 O8 Ca4 -169.8(2) . . . 1_546 ?
Nb4 Ca3 O8 Ca4 179.86(9) 1_556 . . 1_546 ?
Nb3 Ca3 O8 Ca4 -32.35(9) 1_554 . . 1_546 ?
Nb4 Ca3 O8 Ca4 -54.15(18) . . . 1_546 ?
O2 Nb1 O3 Nb2 112.5(4) . . . . ?
O13 Nb1 O3 Nb2 10.9(4) 1_546 . . . ?
O6 Nb1 O3 Nb2 -155.9(4) 3_544 . . . ?
O1 Nb1 O3 Nb2 -82.7(6) . . . . ?
O4 Nb1 O3 Nb2 -69.2(4) 3_545 . . . ?
Ca2 Nb1 O3 Nb2 164.5(4) 1_544 . . . ?
Ca1 Nb1 O3 Nb2 -112.0(4) 3_545 . . . ?
Ca1 Nb1 O3 Nb2 170.5(5) . . . . ?
Ca1 Nb1 O3 Nb2 -20.4(4) 1_556 . . . ?
Ca2 Nb1 O3 Nb2 -15.9(5) 1_545 . . . ?
Ca2 Nb1 O3 Nb2 -97.7(4) 3_544 . . . ?
O2 Nb1 O3 Ca1 -57.93(12) . . . . ?
O13 Nb1 O3 Ca1 -159.57(11) 1_546 . . . ?
O6 Nb1 O3 Ca1 33.63(11) 3_544 . . . ?
O1 Nb1 O3 Ca1 106.8(5) . . . . ?
O4 Nb1 O3 Ca1 120.32(11) 3_545 . . . ?
Ca2 Nb1 O3 Ca1 -5.93(11) 1_544 . . . ?
Ca1 Nb1 O3 Ca1 77.57(11) 3_545 . . . ?
Ca1 Nb1 O3 Ca1 169.09(11) 1_556 . . . ?
Ca2 Nb1 O3 Ca1 173.58(3) 1_545 . . . ?
Ca2 Nb1 O3 Ca1 91.78(10) 3_544 . . . ?
O2 Nb1 O3 Ca2 -149.71(10) . . . 3_544 ?
O13 Nb1 O3 Ca2 108.64(10) 1_546 . . 3_544 ?
O6 Nb1 O3 Ca2 -58.15(11) 3_544 . . 3_544 ?
O1 Nb1 O3 Ca2 15.0(5) . . . 3_544 ?
O4 Nb1 O3 Ca2 28.54(10) 3_545 . . 3_544 ?
Ca2 Nb1 O3 Ca2 -97.71(7) 1_544 . . 3_544 ?
Ca1 Nb1 O3 Ca2 -14.21(12) 3_545 . . 3_544 ?
Ca1 Nb1 O3 Ca2 -91.78(10) . . . 3_544 ?
Ca1 Nb1 O3 Ca2 77.31(7) 1_556 . . 3_544 ?
Ca2 Nb1 O3 Ca2 81.80(10) 1_545 . . 3_544 ?
O2 Nb1 O3 Ca1 132.98(10) . . . 1_556 ?
O13 Nb1 O3 Ca1 31.33(9) 1_546 . . 1_556 ?
O6 Nb1 O3 Ca1 -135.46(9) 3_544 . . 1_556 ?
O1 Nb1 O3 Ca1 -62.3(5) . . . 1_556 ?
O4 Nb1 O3 Ca1 -48.77(8) 3_545 . . 1_556 ?
Ca2 Nb1 O3 Ca1 -175.02(2) 1_544 . . 1_556 ?
Ca1 Nb1 O3 Ca1 -91.52(7) 3_545 . . 1_556 ?
Ca1 Nb1 O3 Ca1 -169.09(11) . . . 1_556 ?
Ca2 Nb1 O3 Ca1 4.49(11) 1_545 . . 1_556 ?
Ca2 Nb1 O3 Ca1 -77.31(7) 3_544 . . 1_556 ?
O5 Nb2 O3 Nb1 -112.8(4) . . . . ?
O7 Nb2 O3 Nb1 -9.6(4) . . . . ?
O4 Nb2 O3 Nb1 155.1(4) . . . . ?
O1 Nb2 O3 Nb1 86.6(6) 1_565 . . . ?
O6 Nb2 O3 Nb1 69.8(4) . . . . ?
Ca2 Nb2 O3 Nb1 -165.7(4) 1_554 . . . ?
Ca1 Nb2 O3 Nb1 111.9(4) 3 . . . ?
Ca2 Nb2 O3 Nb1 17.4(5) . . . . ?
Ca1 Nb2 O3 Nb1 20.4(4) 1_556 . . . ?
Ca1 Nb2 O3 Nb1 -170.5(5) . . . . ?
Ca2 Nb2 O3 Nb1 97.5(4) 3_544 . . . ?
O5 Nb2 O3 Ca1 57.61(12) . . . . ?
O7 Nb2 O3 Ca1 160.84(11) . . . . ?
O4 Nb2 O3 Ca1 -34.45(11) . . . . ?
O1 Nb2 O3 Ca1 -103.0(4) 1_565 . . . ?
O6 Nb2 O3 Ca1 -119.75(11) . . . . ?
Ca2 Nb2 O3 Ca1 4.79(11) 1_554 . . . ?
Ca1 Nb2 O3 Ca1 -77.61(11) 3 . . . ?
Ca2 Nb2 O3 Ca1 -172.19(3) . . . . ?
Ca1 Nb2 O3 Ca1 -169.11(11) 1_556 . . . ?
Ca2 Nb2 O3 Ca1 -92.00(10) 3_544 . . . ?
O5 Nb2 O3 Ca2 149.61(10) . . . 3_544 ?
O7 Nb2 O3 Ca2 -107.16(11) . . . 3_544 ?
O4 Nb2 O3 Ca2 57.54(11) . . . 3_544 ?
O1 Nb2 O3 Ca2 -11.0(5) 1_565 . . 3_544 ?
O6 Nb2 O3 Ca2 -27.76(10) . . . 3_544 ?
Ca2 Nb2 O3 Ca2 96.79(7) 1_554 . . 3_544 ?
Ca1 Nb2 O3 Ca2 14.39(12) 3 . . 3_544 ?
Ca2 Nb2 O3 Ca2 -80.19(10) . . . 3_544 ?
Ca1 Nb2 O3 Ca2 -77.12(7) 1_556 . . 3_544 ?
Ca1 Nb2 O3 Ca2 92.00(10) . . . 3_544 ?
O5 Nb2 O3 Ca1 -133.27(10) . . . 1_556 ?
O7 Nb2 O3 Ca1 -30.05(9) . . . 1_556 ?
O4 Nb2 O3 Ca1 134.66(9) . . . 1_556 ?
O1 Nb2 O3 Ca1 66.1(5) 1_565 . . 1_556 ?
O6 Nb2 O3 Ca1 49.36(9) . . . 1_556 ?
Ca2 Nb2 O3 Ca1 173.91(2) 1_554 . . 1_556 ?
Ca1 Nb2 O3 Ca1 91.50(7) 3 . . 1_556 ?
Ca2 Nb2 O3 Ca1 -3.08(11) . . . 1_556 ?
Ca1 Nb2 O3 Ca1 169.11(11) . . . 1_556 ?
Ca2 Nb2 O3 Ca1 77.12(7) 3_544 . . 1_556 ?
O7 Ca1 O3 Nb1 142.33(10) 1_554 . . . ?
O13 Ca1 O3 Nb1 35.85(13) 1_545 . . . ?
O1 Ca1 O3 Nb1 -91.49(11) 3_554 . . . ?
O4 Ca1 O3 Nb1 -40.32(15) 3_544 . . . ?
O6 Ca1 O3 Nb1 -142.66(9) 1_554 . . . ?
O6 Ca1 O3 Nb1 -26.26(9) 3_544 . . . ?
O4 Ca1 O3 Nb1 -156.43(13) . . . . ?
O9 Ca1 O3 Nb1 88.77(10) 1_554 . . . ?
O3 Ca1 O3 Nb1 89.8(5) 1_554 . . . ?
Nb1 Ca1 O3 Nb1 -126.56(8) 3_554 . . . ?
Nb2 Ca1 O3 Nb1 -56.54(9) 3_544 . . . ?
O7 Ca1 O3 Nb2 -34.19(13) 1_554 . . . ?
O13 Ca1 O3 Nb2 -140.67(10) 1_545 . . . ?
O1 Ca1 O3 Nb2 91.99(11) 3_554 . . . ?
O4 Ca1 O3 Nb2 143.15(9) 3_544 . . . ?
O6 Ca1 O3 Nb2 40.81(15) 1_554 . . . ?
O6 Ca1 O3 Nb2 157.21(13) 3_544 . . . ?
O4 Ca1 O3 Nb2 27.05(9) . . . . ?
O9 Ca1 O3 Nb2 -87.75(10) 1_554 . . . ?
O3 Ca1 O3 Nb2 -86.7(6) 1_554 . . . ?
Nb1 Ca1 O3 Nb2 56.92(9) 3_554 . . . ?
Nb2 Ca1 O3 Nb2 126.93(8) 3_544 . . . ?
O7 Ca1 O3 Ca2 -126.48(8) 1_554 . . 3_544 ?
O13 Ca1 O3 Ca2 127.04(9) 1_545 . . 3_544 ?
O1 Ca1 O3 Ca2 -0.29(7) 3_554 . . 3_544 ?
O4 Ca1 O3 Ca2 50.87(11) 3_544 . . 3_544 ?
O6 Ca1 O3 Ca2 -51.47(12) 1_554 . . 3_544 ?
O6 Ca1 O3 Ca2 64.93(8) 3_544 . . 3_544 ?
O4 Ca1 O3 Ca2 -65.24(7) . . . 3_544 ?
O9 Ca1 O3 Ca2 179.96(8) 1_554 . . 3_544 ?
O3 Ca1 O3 Ca2 -179.0(5) 1_554 . . 3_544 ?
Nb1 Ca1 O3 Ca2 -35.37(5) 3_554 . . 3_544 ?
Nb2 Ca1 O3 Ca2 34.65(5) 3_544 . . 3_544 ?
O7 Ca1 O3 Ca1 -127.5(5) 1_554 . . 1_556 ?
O13 Ca1 O3 Ca1 126.1(5) 1_545 . . 1_556 ?
O1 Ca1 O3 Ca1 -1.3(5) 3_554 . . 1_556 ?
O4 Ca1 O3 Ca1 49.9(6) 3_544 . . 1_556 ?
O6 Ca1 O3 Ca1 -52.5(6) 1_554 . . 1_556 ?
O6 Ca1 O3 Ca1 63.9(5) 3_544 . . 1_556 ?
O4 Ca1 O3 Ca1 -66.2(5) . . . 1_556 ?
O9 Ca1 O3 Ca1 179.0(6) 1_554 . . 1_556 ?
O3 Ca1 O3 Ca1 180.0 1_554 . . 1_556 ?
Nb1 Ca1 O3 Ca1 -36.4(5) 3_554 . . 1_556 ?
Nb2 Ca1 O3 Ca1 33.7(6) 3_544 . . 1_556 ?
O11 Nb4 O14 Ca4 119.1(2) . . . . ?
O9 Nb4 O14 Ca4 26.0(2) 1_564 . . . ?
O12 Nb4 O14 Ca4 -144.9(2) . . . . ?
O13 Nb4 O14 Ca4 -61.5(2) . . . . ?
O2 Nb4 O14 Ca4 -156.1(10) 1_565 . . . ?
Ca4 Nb4 O14 Ca4 118.2(2) 2_575 . . . ?
Ca2 Nb4 O14 Ca4 -107.65(18) 1_554 . . . ?
Ca4 Nb4 O14 Ca4 74.7(2) 1_556 . . . ?
Ca3 Nb4 O14 Ca4 -138.3(3) 1_554 . . . ?
Ca3 Nb4 O14 Ca4 149.28(16) . . . . ?
Ca1 Nb4 O14 Ca4 -26.8(2) 1_565 . . . ?
O11 Nb4 O14 Ca4 0.91(12) . . . 2_575 ?
O9 Nb4 O14 Ca4 -92.16(12) 1_564 . . 2_575 ?
O12 Nb4 O14 Ca4 96.93(11) . . . 2_575 ?
O13 Nb4 O14 Ca4 -179.62(10) . . . 2_575 ?
O2 Nb4 O14 Ca4 85.7(12) 1_565 . . 2_575 ?
Ca2 Nb4 O14 Ca4 134.18(6) 1_554 . . 2_575 ?
Ca4 Nb4 O14 Ca4 -43.43(10) 1_556 . . 2_575 ?
Ca3 Nb4 O14 Ca4 103.58(14) 1_554 . . 2_575 ?
Ca3 Nb4 O14 Ca4 31.11(13) . . . 2_575 ?
Ca1 Nb4 O14 Ca4 -144.96(5) 1_565 . . 2_575 ?
O11 Nb4 O14 Ca3 -102.67(13) . . . 1_554 ?
O9 Nb4 O14 Ca3 164.26(12) 1_564 . . 1_554 ?
O12 Nb4 O14 Ca3 -6.64(13) . . . 1_554 ?
O13 Nb4 O14 Ca3 76.80(13) . . . 1_554 ?
O2 Nb4 O14 Ca3 -17.8(12) 1_565 . . 1_554 ?
Ca4 Nb4 O14 Ca3 -103.58(14) 2_575 . . 1_554 ?
Ca2 Nb4 O14 Ca3 30.60(16) 1_554 . . 1_554 ?
Ca4 Nb4 O14 Ca3 -147.01(8) 1_556 . . 1_554 ?
Ca3 Nb4 O14 Ca3 -72.46(13) . . . 1_554 ?
Ca1 Nb4 O14 Ca3 111.47(10) 1_565 . . 1_554 ?
O8 Ca4 O14 Nb4 -27.3(2) 1_564 . . . ?
O11 Ca4 O14 Nb4 138.5(2) 1_554 . . . ?
O11 Ca4 O14 Nb4 -100.1(2) 2_574 . . . ?
O10 Ca4 O14 Nb4 -10.7(6) 1_563 . . . ?
O14 Ca4 O14 Nb4 -157.87(19) 2_574 . . . ?
O9 Ca4 O14 Nb4 82.8(2) 1_563 . . . ?
Nb4 Ca4 O14 Nb4 -128.5(2) 2_574 . . . ?
Nb3 Ca4 O14 Nb4 61.3(3) 1_563 . . . ?
Nb4 Ca4 O14 Nb4 111.6(2) 1_554 . . . ?
Ca4 Ca4 O14 Nb4 164.60(19) 2_574 . . . ?
Ca4 Ca4 O14 Nb4 -116.1(3) 2_575 . . . ?
O8 Ca4 O14 Ca4 88.83(12) 1_564 . . 2_575 ?
O11 Ca4 O14 Ca4 -105.43(12) 1_554 . . 2_575 ?
O11 Ca4 O14 Ca4 15.95(10) 2_574 . . 2_575 ?
O10 Ca4 O14 Ca4 105.4(4) 1_563 . . 2_575 ?
O14 Ca4 O14 Ca4 -41.79(15) 2_574 . . 2_575 ?
O9 Ca4 O14 Ca4 -161.07(9) 1_563 . . 2_575 ?
Nb4 Ca4 O14 Ca4 -12.38(10) 2_574 . . 2_575 ?
Nb3 Ca4 O14 Ca4 177.43(6) 1_563 . . 2_575 ?
Nb4 Ca4 O14 Ca4 -132.28(9) 1_554 . . 2_575 ?
Ca4 Ca4 O14 Ca4 -79.31(10) 2_574 . . 2_575 ?
O8 Ca4 O14 Ca3 -165.40(10) 1_564 . . 1_554 ?
O11 Ca4 O14 Ca3 0.34(10) 1_554 . . 1_554 ?
O11 Ca4 O14 Ca3 121.72(12) 2_574 . . 1_554 ?
O10 Ca4 O14 Ca3 -148.8(4) 1_563 . . 1_554 ?
O14 Ca4 O14 Ca3 63.98(13) 2_574 . . 1_554 ?
O9 Ca4 O14 Ca3 -55.30(13) 1_563 . . 1_554 ?
Nb4 Ca4 O14 Ca3 93.39(9) 2_574 . . 1_554 ?
Nb3 Ca4 O14 Ca3 -76.80(16) 1_563 . . 1_554 ?
Nb4 Ca4 O14 Ca3 -26.51(10) 1_554 . . 1_554 ?
Ca4 Ca4 O14 Ca3 26.46(11) 2_574 . . 1_554 ?
Ca4 Ca4 O14 Ca3 105.77(14) 2_575 . . 1_554 ?
O8 Nb3 O9 Nb4 1.1(3) . . . 1_546 ?
O10 Nb3 O9 Nb4 102.7(2) . . . 1_546 ?
O12 Nb3 O9 Nb4 -137.8(3) 1_556 . . 1_546 ?
O7 Nb3 O9 Nb4 -90.6(3) . . . 1_546 ?
O5 Nb3 O9 Nb4 -170.5(3) 1_556 . . 1_546 ?
Ca2 Nb3 O9 Nb4 -129.1(2) . . . 1_546 ?
Ca4 Nb3 O9 Nb4 110.5(3) 1_547 . . 1_546 ?
Ca3 Nb3 O9 Nb4 -9.5(3) . . . 1_546 ?
Ca3 Nb3 O9 Nb4 141.6(2) 1_556 . . 1_546 ?
Ca1 Nb3 O9 Nb4 -106.2(3) 1_556 . . 1_546 ?
Ca3 Nb3 O9 Nb4 66.5(2) 2_565 . . 1_546 ?
O8 Nb3 O9 Ca4 -109.44(12) . . . 1_547 ?
O10 Nb3 O9 Ca4 -7.81(12) . . . 1_547 ?
O12 Nb3 O9 Ca4 111.7(4) 1_556 . . 1_547 ?
O7 Nb3 O9 Ca4 158.89(11) . . . 1_547 ?
O5 Nb3 O9 Ca4 78.97(10) 1_556 . . 1_547 ?
Ca2 Nb3 O9 Ca4 120.37(7) . . . 1_547 ?
Ca3 Nb3 O9 Ca4 -120.00(10) . . . 1_547 ?
Ca3 Nb3 O9 Ca4 31.15(10) 1_556 . . 1_547 ?
Ca1 Nb3 O9 Ca4 143.31(13) 1_556 . . 1_547 ?
Ca3 Nb3 O9 Ca4 -43.94(9) 2_565 . . 1_547 ?
O8 Nb3 O9 Ca1 107.25(11) . . . 1_556 ?
O10 Nb3 O9 Ca1 -151.11(12) . . . 1_556 ?
O12 Nb3 O9 Ca1 -31.6(4) 1_556 . . 1_556 ?
O7 Nb3 O9 Ca1 15.58(10) . . . 1_556 ?
O5 Nb3 O9 Ca1 -64.34(10) 1_556 . . 1_556 ?
Ca2 Nb3 O9 Ca1 -22.93(11) . . . 1_556 ?
Ca4 Nb3 O9 Ca1 -143.31(13) 1_547 . . 1_556 ?
Ca3 Nb3 O9 Ca1 96.69(11) . . . 1_556 ?
Ca3 Nb3 O9 Ca1 -112.15(7) 1_556 . . 1_556 ?
Ca3 Nb3 O9 Ca1 172.75(6) 2_565 . . 1_556 ?
O8 Nb3 O10 Ca3 -0.63(16) . . . 2_565 ?
O9 Nb3 O10 Ca3 -103.13(15) . . . 2_565 ?
O12 Nb3 O10 Ca3 93.43(15) 1_556 . . 2_565 ?
O7 Nb3 O10 Ca3 177.7(4) . . . 2_565 ?
O5 Nb3 O10 Ca3 173.72(14) 1_556 . . 2_565 ?
Ca2 Nb3 O10 Ca3 135.43(9) . . . 2_565 ?
Ca4 Nb3 O10 Ca3 -111.21(18) 1_547 . . 2_565 ?
Ca3 Nb3 O10 Ca3 41.93(14) . . . 2_565 ?
Ca3 Nb3 O10 Ca3 140.8(2) 1_556 . . 2_565 ?
Ca1 Nb3 O10 Ca3 -135.36(9) 1_556 . . 2_565 ?
O8 Nb3 O10 Ca3 -141.40(14) . . . 1_556 ?
O9 Nb3 O10 Ca3 116.10(14) . . . 1_556 ?
O12 Nb3 O10 Ca3 -47.34(15) 1_556 . . 1_556 ?
O7 Nb3 O10 Ca3 36.9(6) . . . 1_556 ?
O5 Nb3 O10 Ca3 32.95(12) 1_556 . . 1_556 ?
Ca2 Nb3 O10 Ca3 -5.34(17) . . . 1_556 ?
Ca4 Nb3 O10 Ca3 108.02(16) 1_547 . . 1_556 ?
Ca3 Nb3 O10 Ca3 -98.84(11) . . . 1_556 ?
Ca1 Nb3 O10 Ca3 83.87(15) 1_556 . . 1_556 ?
Ca3 Nb3 O10 Ca3 -140.8(2) 2_565 . . 1_556 ?
O8 Nb3 O10 Ca4 110.58(13) . . . 1_547 ?
O9 Nb3 O10 Ca4 8.08(12) . . . 1_547 ?
O12 Nb3 O10 Ca4 -155.36(12) 1_556 . . 1_547 ?
O7 Nb3 O10 Ca4 -71.1(5) . . . 1_547 ?
O5 Nb3 O10 Ca4 -75.07(11) 1_556 . . 1_547 ?
Ca2 Nb3 O10 Ca4 -113.36(9) . . . 1_547 ?
Ca3 Nb3 O10 Ca4 153.14(8) . . . 1_547 ?
Ca3 Nb3 O10 Ca4 -108.02(16) 1_556 . . 1_547 ?
Ca1 Nb3 O10 Ca4 -24.15(18) 1_556 . . 1_547 ?
Ca3 Nb3 O10 Ca4 111.21(18) 2_565 . . 1_547 ?
O13 Nb1 O2 Nb4 122.1(3) 1_546 . . 1_545 ?
O6 Nb1 O2 Nb4 -62.8(3) 3_544 . . 1_545 ?
O3 Nb1 O2 Nb4 26.6(3) . . . 1_545 ?
O1 Nb1 O2 Nb4 -149.6(3) . . . 1_545 ?
O4 Nb1 O2 Nb4 -129.8(15) 3_545 . . 1_545 ?
Ca2 Nb1 O2 Nb4 -88.6(3) 1_544 . . 1_545 ?
Ca1 Nb1 O2 Nb4 -109.6(3) 3_545 . . 1_545 ?
Ca1 Nb1 O2 Nb4 -11.4(3) . . . 1_545 ?
Ca1 Nb1 O2 Nb4 90.4(3) 1_556 . . 1_545 ?
Ca2 Nb1 O2 Nb4 170.1(3) 1_545 . . 1_545 ?
Ca2 Nb1 O2 Nb4 -17.4(4) 3_544 . . 1_545 ?
O13 Nb1 O2 Ca2 -149.38(10) 1_546 . . 1_544 ?
O6 Nb1 O2 Ca2 25.77(11) 3_544 . . 1_544 ?
O3 Nb1 O2 Ca2 115.21(11) . . . 1_544 ?
O1 Nb1 O2 Ca2 -61.03(12) . . . 1_544 ?
O4 Nb1 O2 Ca2 -41.2(16) 3_545 . . 1_544 ?
Ca1 Nb1 O2 Ca2 -21.01(13) 3_545 . . 1_544 ?
Ca1 Nb1 O2 Ca2 77.19(7) . . . 1_544 ?
Ca1 Nb1 O2 Ca2 178.99(4) 1_556 . . 1_544 ?
Ca2 Nb1 O2 Ca2 -101.31(8) 1_545 . . 1_544 ?
Ca2 Nb1 O2 Ca2 71.17(16) 3_544 . . 1_544 ?
O13 Nb1 O2 Ca3 -33.47(15) 1_546 . . 1_545 ?
O6 Nb1 O2 Ca3 141.68(14) 3_544 . . 1_545 ?
O3 Nb1 O2 Ca3 -128.88(14) . . . 1_545 ?
O1 Nb1 O2 Ca3 54.88(16) . . . 1_545 ?
O4 Nb1 O2 Ca3 74.7(16) 3_545 . . 1_545 ?
Ca2 Nb1 O2 Ca3 115.91(17) 1_544 . . 1_545 ?
Ca1 Nb1 O2 Ca3 94.90(13) 3_545 . . 1_545 ?
Ca1 Nb1 O2 Ca3 -166.90(15) . . . 1_545 ?
Ca1 Nb1 O2 Ca3 -65.10(18) 1_556 . . 1_545 ?
Ca2 Nb1 O2 Ca3 14.60(15) 1_545 . . 1_545 ?
Ca2 Nb1 O2 Ca3 -172.92(4) 3_544 . . 1_545 ?
O7 Nb2 O5 Nb3 -122.5(3) . . . 1_554 ?
O3 Nb2 O5 Nb3 -26.0(3) . . . 1_554 ?
O4 Nb2 O5 Nb3 62.8(3) . . . 1_554 ?
O1 Nb2 O5 Nb3 148.8(3) 1_565 . . 1_554 ?
O6 Nb2 O5 Nb3 120.2(13) . . . 1_554 ?
Ca2 Nb2 O5 Nb3 88.0(3) 1_554 . . 1_554 ?
Ca1 Nb2 O5 Nb3 109.0(3) 3 . . 1_554 ?
Ca2 Nb2 O5 Nb3 -170.4(2) . . . 1_554 ?
Ca1 Nb2 O5 Nb3 -90.1(3) 1_556 . . 1_554 ?
Ca1 Nb2 O5 Nb3 11.5(3) . . . 1_554 ?
Ca2 Nb2 O5 Nb3 17.6(4) 3_544 . . 1_554 ?
O7 Nb2 O5 Ca2 149.47(10) . . . 1_554 ?
O3 Nb2 O5 Ca2 -114.01(11) . . . 1_554 ?
O4 Nb2 O5 Ca2 -25.20(11) . . . 1_554 ?
O1 Nb2 O5 Ca2 60.78(11) 1_565 . . 1_554 ?
O6 Nb2 O5 Ca2 32.2(14) . . . 1_554 ?
Ca1 Nb2 O5 Ca2 21.00(12) 3 . . 1_554 ?
Ca2 Nb2 O5 Ca2 101.58(7) . . . 1_554 ?
Ca1 Nb2 O5 Ca2 -178.08(4) 1_556 . . 1_554 ?
Ca1 Nb2 O5 Ca2 -76.53(7) . . . 1_554 ?
Ca2 Nb2 O5 Ca2 -70.46(15) 3_544 . . 1_554 ?
O7 Nb2 O5 Ca3 31.56(16) . . . . ?
O3 Nb2 O5 Ca3 128.08(14) . . . . ?
O4 Nb2 O5 Ca3 -143.11(14) . . . . ?
O1 Nb2 O5 Ca3 -57.13(15) 1_565 . . . ?
O6 Nb2 O5 Ca3 -85.7(14) . . . . ?
Ca2 Nb2 O5 Ca3 -117.91(16) 1_554 . . . ?
Ca1 Nb2 O5 Ca3 -96.91(13) 3 . . . ?
Ca2 Nb2 O5 Ca3 -16.33(15) . . . . ?
Ca1 Nb2 O5 Ca3 64.01(17) 1_556 . . . ?
Ca1 Nb2 O5 Ca3 165.56(14) . . . . ?
Ca2 Nb2 O5 Ca3 171.63(4) 3_544 . . . ?
O11 Ca3 O5 Nb2 130.27(15) . . . . ?
O8 Ca3 O5 Nb2 -65.22(15) . . . . ?
O10 Ca3 O5 Nb2 -88.2(2) 2_564 . . . ?
O10 Ca3 O5 Nb2 -145.04(18) 1_554 . . . ?
O14 Ca3 O5 Nb2 51.7(2) 1_556 . . . ?
O12 Ca3 O5 Nb2 -0.41(14) 1_556 . . . ?
O2 Ca3 O5 Nb2 86.23(15) 1_565 . . . ?
Nb3 Ca3 O5 Nb2 -35.22(13) . . . . ?
Nb4 Ca3 O5 Nb2 25.90(16) 1_556 . . . ?
Nb3 Ca3 O5 Nb2 -166.9(2) 1_554 . . . ?
Nb4 Ca3 O5 Nb2 124.78(14) . . . . ?
O11 Ca3 O5 Nb3 -62.80(11) . . . 1_554 ?
O8 Ca3 O5 Nb3 101.71(10) . . . 1_554 ?
O10 Ca3 O5 Nb3 78.7(2) 2_564 . . 1_554 ?
O10 Ca3 O5 Nb3 21.89(9) 1_554 . . 1_554 ?
O14 Ca3 O5 Nb3 -141.35(11) 1_556 . . 1_554 ?
O12 Ca3 O5 Nb3 166.52(9) 1_556 . . 1_554 ?
O2 Ca3 O5 Nb3 -106.85(10) 1_565 . . 1_554 ?
Nb3 Ca3 O5 Nb3 131.70(7) . . . 1_554 ?
Nb4 Ca3 O5 Nb3 -167.17(6) 1_556 . . 1_554 ?
Nb4 Ca3 O5 Nb3 -68.29(7) . . . 1_554 ?
O11 Ca3 O5 Ca2 21.05(14) . . . 1_554 ?
O8 Ca3 O5 Ca2 -174.44(13) . . . 1_554 ?
O10 Ca3 O5 Ca2 162.53(16) 2_564 . . 1_554 ?
O10 Ca3 O5 Ca2 105.73(12) 1_554 . . 1_554 ?
O14 Ca3 O5 Ca2 -57.51(16) 1_556 . . 1_554 ?
O12 Ca3 O5 Ca2 -109.64(11) 1_556 . . 1_554 ?
O2 Ca3 O5 Ca2 -23.00(10) 1_565 . . 1_554 ?
Nb3 Ca3 O5 Ca2 -144.45(10) . . . 1_554 ?
Nb4 Ca3 O5 Ca2 -83.33(10) 1_556 . . 1_554 ?
Nb3 Ca3 O5 Ca2 83.85(11) 1_554 . . 1_554 ?
Nb4 Ca3 O5 Ca2 15.56(8) . . . 1_554 ?
O14 Nb4 O13 Nb1 -23.1(2) . . . 1_564 ?
O11 Nb4 O13 Nb1 155.0(3) . . . 1_564 ?
O9 Nb4 O13 Nb1 -124.0(2) 1_564 . . 1_564 ?
O12 Nb4 O13 Nb1 68.0(2) . . . 1_564 ?
O2 Nb4 O13 Nb1 151.1(2) 1_565 . . 1_564 ?
Ca4 Nb4 O13 Nb1 -23.7(3) 2_575 . . 1_564 ?
Ca2 Nb4 O13 Nb1 105.2(2) 1_554 . . 1_564 ?
Ca4 Nb4 O13 Nb1 -143.00(16) 1_556 . . 1_564 ?
Ca3 Nb4 O13 Nb1 18.8(2) 1_554 . . 1_564 ?
Ca3 Nb4 O13 Nb1 122.99(18) . . . 1_564 ?
Ca1 Nb4 O13 Nb1 -146.7(3) 1_565 . . 1_564 ?
O14 Nb4 O13 Ca1 123.54(13) . . . 1_565 ?
O11 Nb4 O13 Ca1 -58.3(5) . . . 1_565 ?
O9 Nb4 O13 Ca1 22.67(12) 1_564 . . 1_565 ?
O12 Nb4 O13 Ca1 -145.27(14) . . . 1_565 ?
O2 Nb4 O13 Ca1 -62.24(12) 1_565 . . 1_565 ?
Ca4 Nb4 O13 Ca1 123.00(12) 2_575 . . 1_565 ?
Ca2 Nb4 O13 Ca1 -108.07(14) 1_554 . . 1_565 ?
Ca4 Nb4 O13 Ca1 3.68(16) 1_556 . . 1_565 ?
Ca3 Nb4 O13 Ca1 165.51(10) 1_554 . . 1_565 ?
Ca3 Nb4 O13 Ca1 -90.32(12) . . . 1_565 ?
O14 Nb4 O13 Ca2 -128.39(11) . . . 1_554 ?
O11 Nb4 O13 Ca2 49.7(4) . . . 1_554 ?
O9 Nb4 O13 Ca2 130.73(12) 1_564 . . 1_554 ?
O12 Nb4 O13 Ca2 -37.21(11) . . . 1_554 ?
O2 Nb4 O13 Ca2 45.83(10) 1_565 . . 1_554 ?
Ca4 Nb4 O13 Ca2 -128.93(10) 2_575 . . 1_554 ?
Ca4 Nb4 O13 Ca2 111.75(8) 1_556 . . 1_554 ?
Ca3 Nb4 O13 Ca2 -86.43(7) 1_554 . . 1_554 ?
Ca3 Nb4 O13 Ca2 17.75(13) . . . 1_554 ?
Ca1 Nb4 O13 Ca2 108.07(14) 1_565 . . 1_554 ?
O14 Nb4 O12 Nb3 -104.6(4) . . . 1_554 ?
O11 Nb4 O12 Nb3 -8.1(4) . . . 1_554 ?
O9 Nb4 O12 Nb3 108.5(5) 1_564 . . 1_554 ?
O13 Nb4 O12 Nb3 155.7(4) . . . 1_554 ?
O2 Nb4 O12 Nb3 74.2(4) 1_565 . . 1_554 ?
Ca4 Nb4 O12 Nb3 -56.1(4) 2_575 . . 1_554 ?
Ca2 Nb4 O12 Nb3 117.6(4) 1_554 . . 1_554 ?
Ca4 Nb4 O12 Nb3 11.2(4) 1_556 . . 1_554 ?
Ca3 Nb4 O12 Nb3 -110.6(4) 1_554 . . 1_554 ?
Ca3 Nb4 O12 Nb3 19.0(3) . . . 1_554 ?
Ca1 Nb4 O12 Nb3 133.7(3) 1_565 . . 1_554 ?
O14 Nb4 O12 Ca2 137.81(13) . . . 1_554 ?
O11 Nb4 O12 Ca2 -125.66(12) . . . 1_554 ?
O9 Nb4 O12 Ca2 -9.1(5) 1_564 . . 1_554 ?
O13 Nb4 O12 Ca2 38.17(11) . . . 1_554 ?
O2 Nb4 O12 Ca2 -43.31(11) 1_565 . . 1_554 ?
Ca4 Nb4 O12 Ca2 -173.62(8) 2_575 . . 1_554 ?
Ca4 Nb4 O12 Ca2 -106.34(10) 1_556 . . 1_554 ?
Ca3 Nb4 O12 Ca2 131.80(14) 1_554 . . 1_554 ?
Ca3 Nb4 O12 Ca2 -98.57(10) . . . 1_554 ?
Ca1 Nb4 O12 Ca2 16.14(12) 1_565 . . 1_554 ?
O14 Nb4 O12 Ca3 6.01(12) . . . 1_554 ?
O11 Nb4 O12 Ca3 102.54(12) . . . 1_554 ?
O9 Nb4 O12 Ca3 -140.9(4) 1_564 . . 1_554 ?
O13 Nb4 O12 Ca3 -93.63(10) . . . 1_554 ?
O2 Nb4 O12 Ca3 -175.11(10) 1_565 . . 1_554 ?
Ca4 Nb4 O12 Ca3 54.59(8) 2_575 . . 1_554 ?
Ca2 Nb4 O12 Ca3 -131.80(14) 1_554 . . 1_554 ?
Ca4 Nb4 O12 Ca3 121.87(10) 1_556 . . 1_554 ?
Ca3 Nb4 O12 Ca3 129.63(9) . . . 1_554 ?
Ca1 Nb4 O12 Ca3 -115.66(6) 1_565 . . 1_554 ?
O2 Nb1 O1 Nb2 16.5(3) . . . 1_545 ?
O13 Nb1 O1 Nb2 117.3(2) 1_546 . . 1_545 ?
O6 Nb1 O1 Nb2 -74.9(2) 3_544 . . 1_545 ?
O3 Nb1 O1 Nb2 -148.3(4) . . . 1_545 ?
O4 Nb1 O1 Nb2 -162.0(2) 3_545 . . 1_545 ?
Ca2 Nb1 O1 Nb2 -30.3(2) 1_544 . . 1_545 ?
Ca1 Nb1 O1 Nb2 -113.1(3) 3_545 . . 1_545 ?
Ca1 Nb1 O1 Nb2 -56.6(3) . . . 1_545 ?
Ca1 Nb1 O1 Nb2 154.3(2) 1_556 . . 1_545 ?
Ca2 Nb1 O1 Nb2 130.4(3) 1_545 . . 1_545 ?
Ca2 Nb1 O1 Nb2 -135.1(2) 3_544 . . 1_545 ?
O2 Nb1 O1 Ca2 -113.87(12) . . . 1_545 ?
O13 Nb1 O1 Ca2 -13.12(11) 1_546 . . 1_545 ?
O6 Nb1 O1 Ca2 154.75(12) 3_544 . . 1_545 ?
O3 Nb1 O1 Ca2 81.3(5) . . . 1_545 ?
O4 Nb1 O1 Ca2 67.63(11) 3_545 . . 1_545 ?
Ca2 Nb1 O1 Ca2 -160.68(11) 1_544 . . 1_545 ?
Ca1 Nb1 O1 Ca2 116.57(14) 3_545 . . 1_545 ?
Ca1 Nb1 O1 Ca2 173.00(4) . . . 1_545 ?
Ca1 Nb1 O1 Ca2 23.93(10) 1_556 . . 1_545 ?
Ca2 Nb1 O1 Ca2 94.53(9) 3_544 . . 1_545 ?
O2 Nb1 O1 Ca1 129.56(12) . . . 3_545 ?
O13 Nb1 O1 Ca1 -129.69(12) 1_546 . . 3_545 ?
O6 Nb1 O1 Ca1 38.17(12) 3_544 . . 3_545 ?
O3 Nb1 O1 Ca1 -35.3(6) . . . 3_545 ?
O4 Nb1 O1 Ca1 -48.94(11) 3_545 . . 3_545 ?
Ca2 Nb1 O1 Ca1 82.75(9) 1_544 . . 3_545 ?
Ca1 Nb1 O1 Ca1 56.43(15) . . . 3_545 ?
Ca1 Nb1 O1 Ca1 -92.64(9) 1_556 . . 3_545 ?
Ca2 Nb1 O1 Ca1 -116.57(14) 1_545 . . 3_545 ?
Ca2 Nb1 O1 Ca1 -22.04(12) 3_544 . . 3_545 ?

_diffrn_measured_fraction_theta_max 0.992
_diffrn_reflns_theta_full        27.51
_diffrn_measured_fraction_theta_full 0.992
_refine_diff_density_max         0.583
_refine_diff_density_min         -0.648
_refine_diff_density_rms         0.126
